Share this document with a friend

Embed Size (px)

of 149
/149

Transcript

Strongly Disordered S-Wave Superconductors

A Thesis

for the degree of Doctor of Philosophy

in Physics

Tata Institute of Fundamental Research

Mumbai

To my parents

This thesis is a presentation of my original research work.

Wherever contributions of others are involved, every effort is

made to indicate this clearly, with due reference to the literature,

and acknowledgement of collaborative research and discussions.

The work was done under the guidance of Professor Pratap

Raychaudhuri, at the Tata Institute of Fundamental Research,

Mumbai.

Anand Kamlapure

In my capacity as supervisor of the candidate’s thesis, I certify

that the above statements are true to the best of my knowledge.

Prof. Pratap Raychaudhuri

STATEMENT OF JOINT WORK

The experiments reported in this thesis have been carried out in the Department

of Condensed Matter Physics and Material Science under the guidance of Prof. Pratap

Raychaudhuri. The results of the major portions of the work presented in this thesis

have already been published in refereed journals.

Most of the experiments discussed in this thesis have been conducted by me in

the department. For completeness, I have included some of the experiments and data

analysis performed by other group members and collaborators.

Some of the scanning tunneling measurements were carried out jointly with

Garima Saraswat and Somesh Chandra Ganguli. Transport, Magnetoresistance and

Hall effect measurements were carried out in collaboration with Madhavi Chand.

Penetration depth measurements were carried out by Mintu Mondal and Sanjeev

Kumar. All the Transmission Electron Microscope measurements were carried out by

Tanmay Das and Somnath Bhattacharyya. Theoretical work was done in collaboration

with Dr. Vikram Tripathi of Department of Theoretical Physics, TIFR and Dr. Lara

Benfatto and Dr. Gabriel Lemarié of University of Rome, Rome, Italy.

PREFACE

The work presented in this thesis is on the experimental investigation of the

effect of disorder on s-wave superconductor NbN through scanning tunneling

spectroscopy (STS) measurements.

Disorder induced superconductor insulator transition (SIT) has been the subject

of interest since decades and there have been major advances both experimentally and

theoretically in understanding the nature of SIT. Recently new insights have been

offered by the numerical simulations which predicts unprecedented phenomena such

as persistence of gap across the SIT, spatial inhomogeneity in the gap and order

parameter, emergence of superconductivity over much larger length scale than the

disorder length scale, which needs to be addressed through sophisticated experiments.

The work presented in this thesis unravels many of these novel phenomena near the

SIT in s-wave superconductor, NbN, primarily through scanning tunneling

spectroscopy measurements and supported by results of penetration depth and transport

measurements.

The thesis is organized in following way, In Chapter 1, I will introduce the

motivation for our experiments on disordered superconductors through the advances in

the experimental and theoretical works. I will also introduce our model system: NbN

as a perfect system and its characterization through transmission electron microscope

at the atomic scale. In Chapter 2, I will elaborate on the basics of scanning tunneling

microscope (STM), fabrication of low temperature STM, related techniques and the

scheme of measurements. Chapter 3 focuses on our observation of formation of

pseudogap state in NbN in presence of strong disorder. We argue that the phase

fluctuation is the possible mechanism for the formation of pseudogap state. In Chapter

4, we investigate the ground state superconducting properties in strongly disordered

NbN through spatially resolved STS measurements. We identify that the coherence

peak height is a measure of local order parameter and show that the superconductivity

in the disordered NbN emerges over tens of nanometer scale while the structural

disorder present in the system is at atomic scale. In this chapter we also show that the

order parameter distribution in strongly disordered NbN has a universal behaviour

irrespective of the strength of disorder present in the system. We end the chapter with

the temperature evolution of inhomogeneous superconducting state through spatially

resolved STS measurements. In the concluding Chapter 5, I will summarize all our

investigation during past 6 years and present a phase diagram showing evolution of

various energy scales with disorder.

ACKNOWLEDGEMENTS

First and foremost, I would like to express my sincere gratitude to my thesis

advisor Prof. Pratap Raychaudhuri for the continuous support for my PhD work, for his

patience, motivation and enthusiasm.

I thank my fellow lab mates Garima Saraswat, Madhavi Chand, Mintu Mondal,

Sanjeev Kumar, Archana Mishra, Somesh Chandra Ganguli, Rini Ganguly, Harkirat

Singh, Prashant Shirage, John Jesudasan and Vivas Bagwe for their constant help and

support in every regard.

My sincere thanks goes to Subash Pai from Excel Instruments for all the prompt

technical support. I also thank Bhagyashree (Shilpa) Chalke, Rudhir Bapat, Nilesh

Kulkarni for the help in characterizing the samples and Atul Raut for technical help.

Most importantly I thank Low Temperature Facility team of TIFR for continuous

supply of liquid He and Nitrogen.

I also thank Vikram Tripathi, Lara Benfatto, Gabriel Lemarié for all the

discussions and theoretical support.

I take the opportunity to thank all my friends for their support, motivation and

all the fun we had during my Phd, especially I would like mention Sachin, Jaysurya,

Ajith, Gajendra, Abhishek, Nilesh, Harshad, Nikesh, Ashish, Amlan, Laskar, Bhanu,

Pranab, Abhishek, Mohon, Ronjoy, Sayanti, Anuj, Shishram, Vinod, Subhash, Amar,

Sunil, Abhijeet, Vinod, Jay, Jay, Sanjiv, Onkar, Shireen, Amul, Rajkiran, Lasse and

Pavel.

I finally thank my family members for their love and patience and I dedicate

this thesis to my parents.

LIST OF PUBLICATIONS

In refereed Journal and related to material presented here.

1. Emergence of nanoscale inhomogeneity in the superconducting state of a

homogeneously disordered conventional superconductor

Bhattacharya and Pratap Raychaudhuri

Scientific Reports 3 , 2979 (2013).

2. A 350 mK, 9 T scanning tunneling microscope for the study of superconducting

thin films and single crystals

Anand Kamlapure, Garima Saraswat, Somesh Chandra Ganguli, Vivas Bagwe,

Pratap Raychaudhuri and Subash P. Pai

Rev. Sci. Instrum. 84, 123905.

3. Universal scaling of the order-parameter distribution in strongly disordered

superconductors

G. Lemarié, A. Kamlapure, D. Bucheli, L. Benfatto, J. Lorenzana, G. Seibold, S.

C. Ganguli, P. Raychaudhuri and C. Castellani

Phys. Rev. B 87, 184509 (2013).

4. Phase diagram of the strongly disordered s-wave superconductor NbN close to the

metal-insulator transition

Madhavi Chand, Garima Saraswat, Anand Kamlapure, Mintu Mondal, Sanjeev

Kumar, John Jesudasan, Vivas Bagwe, Lara Benfatto, Vikram Tripathi, and Pratap

Raychaudhuri

Phys. Rev. B 85, 014508 (2012).

5. Phase Fluctuations in a Strongly Disordered s-Wave NbN Superconductor Close to

the Metal-Insulator Transition

Kumar, John Jesudasan, L. Benfatto, Vikram Tripathi, and Pratap Raychaudhuri

Phys. Rev. Lett. 106, 047001 (2011).

6. Enhancement of the finite-frequency superfluid response in the pseudogap regime

of strongly disordered superconducting films

Mintu Mondal, Anand Kamlapure, Somesh Chandra Ganguli, John Jesudasan,

Vivas Bagwe, Lara Benfatto and Pratap Raychaudhuri

Scientific Reports 3, 1357 (2013).

7. Temperature dependence of resistivity and Hall coefficient in strongly disordered

NbN thin films

Madhavi Chand, Archana Mishra, Y. M. Xiong, Anand Kamlapure, S. P.

Chockalingam, John Jesudasan, Vivas Bagwe, Mintu Mondal, P. W. Adams,

Vikram Tripathi, and Pratap Raychaudhuri

Phys. Rev. B 80, 134514 (2009).

8. Tunneling studies in a homogeneously disordered s-wave superconductor: NbN

S. P. Chockalingam, Madhavi Chand, Anand Kamlapure, John Jesudasan, Archana

Mishra, Vikram Tripathi, and Pratap Raychaudhuri

Phys. Rev. B 79, 094509 (2009).

In refereed journals, not related to the work presented

here.

1. Measurement of magnetic penetration depth and superconducting energy gap in

very thin epitaxial NbN films

Anand Kamlapure, Mintu Mondal, Madhavi Chand, Archana Mishra, John

Jesudasan, Vivas Bagwe, L. Benfatto, Vikram Tripathi, and Pratap Raychaudhuri

Appl. Phys. Lett. 96, 072509 (2010).

2. Andreev bound state and multiple energy gaps in the noncentrosymmetric

superconductor, BiPd

Mintu Mondal, Bhanu Joshi, Sanjeev Kumar, Anand Kamlapure, Somesh Chandra

Ganguli, Arumugam Thamizhavel, Sudhansu S. Mandal, Srinivasan Ramakrishnan

and Pratap Raychaudhuri

3. Role of the Vortex-Core Energy on the Berezinskii-Kosterlitz-Thouless Transition

in Thin Films of NbN

Mintu Mondal, Sanjeev Kumar, Madhavi Chand, Anand Kamlapure, Garima

Saraswat, G. Seibold, L. Benfatto, and Pratap Raychaudhuri

Phys. Rev. Lett. 107, 217003 (2011).

Conference Proceedings

1. Pseudogap state in strongly disordered conventional superconductor, NbN

Anand Kamlapure, Garima Saraswat, Madhavi Chand, Mintu Mondal, Sanjeev

Kumar, John Jesudasan, Vivas Bagwe, Lara Benfatto, Vikram Tripathi and Pratap

Raychaudhuri

J. Phys.: Conf. Ser. 400 022044 (2012).

2. Study of Pseudogap State in NbN using Scanning Tunneling Spectroscopy

Madhavi Chand, Anand Kamlapure, Garima Saraswat, Sanjeev Kumar, John

Jesudasan, Mintu Mondal, Vivas Bagwe, Vikram Tripathi, Pratap Raychaudhuri.

AIP Conference Proceedings 1349, 61.

3. Upper Critical Field and Coherence Length of Homogenously Disordered Epitaxial

3-Dimensional NbN Films

Kumar, Garima Saraswat, Vivas C Bagwe, Vikram Tripathi, Pratap Raychaudhuri

AIP Conference Proceedings 1349, 923.

4. Magnetoresistance studies of homogenously disordered 3-dimensional NbN thin

films

Saraswat, SP Chockalingam, John Jesudasan, Vivas Bagwe, Vikram Tripathi, Lara

Benfatto, Pratap Raychaudhuri

Films

Saraswat, Vivas C Bagwe, John Jesudasan, Lara Benfatto, Pratap Raychaudhuri

Journal of Physics: Conference Series 400 (2), 022078.

6. Effect of Phase Fluctuations on the Superconducting Properties of Strongly

Disordered 3D NbN Thin Films

Madhavi Chand, Mintu Mondal, Anand Kamlapure, Garima Saraswat, Archana

Mishra, John Jesudasan, Vivas C Bagwe, Sanjeev Kumar, Vikram Tripathi, Lara

Benfatto, Pratap Raychaudhuri

TABLE OF CONTENTS

1.1.C Nonlocal Response: Pippard Coherence length ( ξ0 ) ............... 46

1.1.D Ginzburg Landau (G-L) model of superconductivity ................ 47

Phase stiffness ............................................................................ 48

Type I and Type II superconductors .......................................... 49

1.1.E BCS theory of superconductivity ........................................................ 50

The gap function ........................................................................ 51

BCS density of states .................................................................. 52

1.1.F Electron tunneling and measurement of .................................... 53

1.2 Disordered Superconductors ........................................................................ 54

1.3.A Sample growth and introducing disorder...................................... 56

1.3.B Structural characterization of NbN films ....................................... 57

1.3.C Quantification of disorder ...................................................................... 58

1.4 Effects of disorder .............................................................................................. 58

1.4.A Resistivity and measurement of Tc.................................................... 59

1.4.B Hall carrier density measurement ..................................................... 60

1.4.C Upper critical field (Hc2) and coherence length (ξGL) ................ 61

1.4.D Magnetic penetration depth (λ).......................................................... 61

2.2 STM Theory ............................................................................................................71

2.3.A STM Head .......................................................................................................78

Coarse positioner: ...................................................................... 78

Piezoelectric tube ...................................................................... 80

Calibration of Piezo constants ................................................... 83

Tip preparation .......................................................................... 84

2.3.B Sample holder ..............................................................................................85

2.3.E 3He Cryostat ..................................................................................................89

Vibrational noise ........................................................................ 91

Electrical noise ........................................................................... 93

Normal Superconductor tunneling ............................................ 97

Conductance map ...................................................................... 99

2.5 Reference ............................................................................................................. 101

Chapter 3 ........................................................................................... 106

3.1.A In-situ preparation of NbN films ...................................................... 107

3.1.B Line scan and averaged spectrum .................................................. 108

3.1.C DOS evolution with temperature .................................................... 109

3.1.D Background correction for disorder NbN samples ................ 109

3.2 Experimental results ...................................................................................... 111

Regime III Nonsuperconducting regime ................................... 119

3.4 Summary .............................................................................................................. 120

3.5 References ........................................................................................................... 121

Chapter 4 .......................................................................................... 125

4.1 Introduction ....................................................................................................... 125

4.2 Investigation of structural disorder in NbN at the atomic scale.

......................................................................................................................................................... 126

......................................................................................................................................................... 129

4.5 Coherence peak height as a measure of local order parameter 130

4.6 Emergence of inhomogeneity in the superconducting state ...... 133

4.7 Universal scaling of the order parameter distribution .................. 135

4.8 Temperature evolution of the inhomogeneous superconduct .. 137

4.9 Discussion ............................................................................................................ 141

4.10 Summary ........................................................................................................... 142

4.11 References ........................................................................................................ 144

Chapter 5 .......................................................................................... 147

a lattice constant or characteristic length scale of phase fluctuations

e electronic charge

EF Fermi energy

Hc2 upper critical field

J superfluid stiffness

kB Boltzmann constant

kF Fermi wave-number

Mαβ Tunneling matrix element between the states α and β

n number density/ electronic carrier density

ns superfluid density

R resistance

resistivity

DOS density of states

HRTEM high resolution transmission electron microscope

HTSC high temperature superconductors

IVC inner vacuum chamber

MIT metal-insulator transition

Chapter 1. Introduction:

The interplay of superconductivity and disorder is one of the most intriguing problems

of quantum many body physics. Superconducting pairing interactions in a normal metal

drives the system into a phase coherent state with zero electrical resistance. In contrast,

in a normal metal increasing disorder progressively increases the resistance through

disorder scattering eventually giving rise to an insulator at high disorder where all

electronic states are localized. Quite early on, it was argued by Anderson1 that since

BCS superconductors respect time reversal symmetry, superconductivity is robust

against nonmagnetic impurities and the critical temperature Tc is not affected by such

disorder. However experiments showed that strong disorder reduces Tc and ultimately

drives the system into an insulator2. Various other phenomena are observed in the

vicinity of Superconductor Insulator transition (SIT) which includes the giant peak in

the magnetoresistance in thin films3, magnetic flux quantization in nano-honeycomb

patterned insulating thin films of Bi4, finite high frequency superfluid stiffness above

Tc in amorphous InOx films5, finite spectral gap in the conductance spectra much above

Tc in scanning tunneling microscope (STM) experiments6,7,8 etc. All of these points

towards the existence of finite superconducting correlation persisting in the system

even though the global superconductivity is destroyed due to disorder.

In recent times numerous theories and numerical simulations have been carried

out in order to understand the real space evolution of superconductivity in presence of

strong disorder. In the intermediate disorder limit the effect of disorder is to decrease

the pairing amplitude9 through an increase in the electron-electron Coulomb repulsion

which results in decrease in Tc. On the insulating side of SIT, it has been argued that

Cooper pair exists even after the single electrons states are completely localized10. The

numerical simulations involve solving Attractive Hubbard model with random on-site

energy11,12,13. Although these simulations ignore the Coulomb interactions and are done

on relatively small lattice the end results are instructive. These simulations indicate that

in the presence of strong disorder the superconducting order parameter becomes

inhomogeneous, spontaneously segregating into superconducting domains, dispersed

in an insulating matrix. Consequently the energy gap, Δ, is not strongly affected but the

energy cost of spatially twisting the phase of the condensate, superfluid stiffness J,

22 Synopsis

decreases rapidly with increasing disorder making the system more susceptible to phase

fluctuations. Thus, in presence of strong disorder near SIT, system consists of

superconducting islands and their phases are Josephson coupled through insulating

regions. Another interesting consequence of these simulations is that in presence of

strong disorder with lowering temperature, Copper pairs are formed above the Tc but

they are phase incoherent. Therefore one expects a resistive state but finite gap due to

superconducting correlations in the local density of states. This gap is termed as

pseudogap which resembles well established pseudogap in high Tc Cuprates.

1.1 Our model system: NbN

For our investigation we use thin films of NbN as a model for the study of effect

of disorder which can be grown by sputtering Nb in Ar + N2 gas mixture. NbN is s-

wave superconductor with relatively high Tc ~16K. Films are grown on single

crystalline MgO substrates and are highly epitaxial. All the films grown for the study

have thickness > 50nm which is much larger than the dirty limit coherence length x~5-

8 nm14 and can be considered to be 3D as far as superconducting correlations are

concerned. Disorder in the film can be tuned by varying the deposition conditions:

either by decreasing the sputtering power or by increasing N2 in the gas mixture15,16.

Disorder in the samples is characterized by Ioffe-Regel parameter, kFl, using the

formula

(1)

where RH is the Hall resistance and ρ is the resistivity, both of which are

measured using transport measurements. While our most ordered sample shows Tc

~16K, with increasing disorder Tc monotonically decreases all the way down to

<300mK. The range of kFl varies from 1 to 10.2 in our samples.

1.2 Structural characterization of disorder

Thin films of NbN grown using sputtering method show high degree of epitaxy

revealed through transmission electron microscopy (TEM) images17. Fig.1 (a) and (d)

show high resolution TEM images probed at the interface of MgO substrate and NbN

film along <110> direction for the two samples with Tc = 16K and 2.5K respectively.

Synopsis 23

The difference between the two films becomes prominent when we take high

resolution scanning TEM data (HRSTEM) as shown in Fig. 1. Panels (b) and (e) shows

HRSTEM image for the two samples with Tc = 16K and 2.5K and panels (c) and (f)

show corresponding two dimensional intensity distribution plots. Intensity in the

HRSTEM image is primarily contributed by Nb and is proportional to the number of

Nb atoms in the probing column. Smooth intensity variation in clean sample (Tc = 16K)

shows the overall thickness variation produced during ion beam milling while the

disordered sample (Tc = 2.5K) shows random distribution of intensity in the columns

showing random number of Nb atoms in the adjacent columns. This clearly shows that

for the disordered films, the lattice contains Nb vacancies but when probed at the large

scale it is homogeneous. Thus we have an ideal system in which disorder is present at

the atomic length scale and the disorder is homogeneous over entire film.

All the work presented in this thesis on disordered NbN is primarily carried out

in our home built STM. Details of the STM and measurement techniques are discussed

in the next chapter.

K

Figure 1 TEM images (a), (d) High resolution TEM images for samples with Tc = 16K and

2.5K respectively. (b), (e) corresponding high resolution scanning TEM images. (c), (f)

surface plots of 2 dimensional intensity distributions corresponding to (b) and (e)

respectively.

Chapter 2. Scanning tunneling microscope

Scanning tunneling microscope (STM) is a powerful tool to probe the electronic

structure of the material at the atomic scale. It works on the principle of quantum

mechanical tunneling between two electrodes through vacuum as a barrier. Essential

parts consist of a sharp metallic tip which is brought near the sample using positioning

units. Small bias applied between tip and sample make the tunneling current flow

between them which is amplified and recorded. Tunneling current exponentially

depends on the distance between tip and sample. By keeping the current constant,

distance between the tip and sample is held constant using feedback loop and by

scanning over the sample the topographic image of the sample is generated.

2.1 Setup

The overall schematic of our system is shown in Fig. 2(a). The assembly

primarily consists of three units, Sample preparation chamber, load lock and the 4He

dewar18. Sample preparation chamber comprises of two magnetron sputtering guns, two

Figure 2 (a) Schematic view of the home built low temperature scanning tunneling

microscope. Cryostat and magnet have been made semi-transparent to show the

internal construction. (b) Schematic view of the STM head shown along with the sample

holder.

Synopsis 25

evaporation sources, a plasma ion etching gun and a heater to heat the sample during

the deposition. Load lock chamber serves as the stage to transfer sample from

deposition chamber into the STM chamber using a pair of transfer manipulators. 4He

dewar has a 9T magnet which houses 3He insert. Helium cryostat hangs from custom

designed vibration isolation table mounted on pneumatic legs and consists of variable

temperature insert (VTI) and STM head. STM head (Fig. 2(b)) attached to the VTI

consists of sample housing assembly, positioning unit and printed circuit board for the

electrical connections. A combination of active and passive vibration isolation systems

are used to obtain the required mechanical stability of the tip. The entire system

operates in a high vacuum of 10-7 mbar and the base temperature for the measurements

is 350mK. Commercially bought control electronics and data acquisition unit (R9,

RHK Technology) is used carry out our experiments.

2.2 Methods

Thin films are grown on substrate mounted on specially designed sample holder

made of Molybdenum. The Molybdenum holder has threading on side and bottom for

holding on the manipulators. Substrate is secured in place on the holder using a cap

which also provides electrical contact with the sample for STM measurements. To

ensure electrical contact between film and holder (Fig. 3) substrate is pre-deposited

with NbN strips in another chamber and the actual film is grown on this strip in STM

chamber. Once the film is grown the

sample holder attached on

horizontal manipulator is pulled

with the vertical manipulator. Using

vertical manipulator the sample

temperature radiation coming from

of set of metal discs mounted on

steel rod is inserted in the annular

Figure 3 Design of sample holder (a)

Molybdenum cap, (b) Substrate with strip

deposited at the edge, (c) Molybdenum sample

holder, (d) Sample holder assembly, showing

substrate fastened with cap. (e) Resulting film

on the substrate after the deposition.

26 Synopsis

region of VTI. Once all the measurements are completed on the sample it is taken out

from the STM and resistivity versus temperature is measured in different cryostat.

2.3 Scanning tunneling spectroscopy

Another powerful technique using STM is to measure local density of states

through tunneling conductance measurements and the method is called as scanning

tunneling spectroscopy (STS). The tunneling conductance (G(V)) between the normal

metal tip and the superconductor is given by19,

() ∝ 1

∫ () (−

( − )

(2)

It can be shown that at sufficiently low temperatures Fermi function becomes

step function and () ∝ () i.e. the tunneling conductance is proportional to the

local density of states of the sample at energy E = eV. To measure the tunneling

conductance, tip sample distance is fixed by switching off the feedback loop and a small

alternating voltage is modulated on the bias. The resultant amplitude of the current

modulation as read by the lock-in amplifier is proportional to the / as can be seen

by Taylor expansion of the current,

( + sin()) ≈ () +

| . sin() (3)

The modulation voltage used in the measurement is = 150 and the

frequency used is 419.3Hz.

Temperature evolution of tunneling density of states (DOS) is investigated

through STS measurements along a line. Averaged spectra at different temperatures are

obtained by taking the average of about 20 spectra each at 32 equidistant points over

the line of length 200 nm and then averaging all in once. The ground state

superconducting properties and its temperature evolution are measured through

spatially resolved STS data. To acquire such data initially topography is imaged at

lowest temperature and then by defining a grid of 32×32 STS data is acquired at each

location (typically 5 spectra at each pixel and then averaged). For higher temperatures

we match the topography before acquiring spatially resolved STS data.

Synopsis 27

NbN

One of the most curious and debated state is the pseudogap state observed in

high Tc superconductors where finite gap in the DOS at Fermi level is observed much

above the superconducting transition temperature which evolves continuously from the

superconducting energy gap below Tc. Several scenarios based either on peculiarities

specific to High Tc Cuprates such as an order competing with superconductivity, or a

superconducting transition driven by phase fluctuations have been suggested as

possible origin of this feature. In this section we elucidate formation of pseudogap state

in NbN using scanning tunneling spectroscopy.

In strong disorder limit all the samples show two distinct features in tunneling

spectra: A low bias dip close to Fermi level which is associated with superconductivity

and a weakly temperature dependent V-shaped background which extends up to high

bias. This second feature which persists up to the highest temperature of our

measurements arises from the Altshuler-Aronov (A-A) type e-e interactions in the

normal state20. To extract the superconducting information from this data we divide the

low temperature spectra by the spectra at sufficiently high temperature where we do

not have any soft gap due to superconducting correlations. The temperature up to which

the pseudogap persists is defined as T*.

-3 -2 -1 0 1 2 3

0.7

0.8

0.9

1.0

4.4K

4.04K

3.61K

3.3K

3.1K

2.6K

0.8

0.9

-1.5

0.0

1.5

3.0

T*

V (

-100

0

100

3.1K

3.3K

3.61K

4.04K

5.33K

7K

9.35K

9.35K

8K

7K

6.28K

5.33K

4.84K

d v

V (mV)

Figure 4 (a) Normalized conductance curves for the sample with Tc=2.6K.

(b) Derivatives of the conductance curves in panel (a). Few curves are

removed for clarity. (c) Normalized conductance curves after dividing

curves in panel (a) from 9.35K data. (d) Surface plot of the curves of panel

(c)

28 Synopsis

Representative data for one of the strongly disordered samples (Tc = 2.6K) is

shown in Fig. 4. Fig. 4(a) shows conductance spectra at different temperatures. We

observe that the low bias gap feature disappears above 8K and the spectrum at 9.35K

has only the broad background. This is clearly seen in the dG(V)/dV versus V curves

(Fig. 4(b)) where the symmetric peak-dip structure associated with the low bias feature

completely disappears for the spectrum at 9.35K. Therefore to remove the A-A

background from the low temperature spectra we divide the spectrum at 9.35K. Fig.4(c)

shows the divided spectra and Fig. 4 (d) shows the colormap of divided data with x-

axis as the temperature, y-axis as the bias and the colorscale as the normalized

conductance value. The data in panel (d) shows that the pseudogap persists up to 6.5K

i.e. T* = 6.5K.

Series of NbN films with increasing disorder were studied using STS. Fig. 5

shows the temperature evolution of tunneling DOS for four samples with Tc = 11.9K,

6K, 2.9K and 1.65K in the form of colormap. All the plots in this figure are corrected

for Altshuler-Aronov background. R-T data for the same sample is indicated by thick

line on top of each colormap. Representative spectra at three temperatures are shown

to the right for clarity. Panel (a) Tc = 11.9K, shows that at low temperature spectra

consist of dip close to zero bias and two symmetric peaks consistent with BCS density

of states. The gap in the spectra vanishes exactly at Tc in accordance with BCS theory

and flat metallic DOS is restored for T > Tc. For the sample with Tc = 6K the gap

remains finite upto slightly higher temperature. For strongly disordered samples (Tc =

2.9K and 1.65K) the gap in the electronic spectra at the Fermi level persists all the way

upto ~7K showing that it forms the pseudogap state and the corresponding T*~ 7K.

Thus we observe that in presence of weak disorder gap closes exactly at Tc while for

strong disorder NbN forms a pseudogapped state above Tc.

Observation of pseudogapped state can be explained using phase fluctuation

scenario. Superconducting order is characterized by complex order parameter given by

Δ0eiφ, where Δ0 is amplitude of the order parameter (which is proportional to the

superconducting energy gap) and φ is the phase, which is same for the entire sample in

the superconducting state. The loss of superconductivity can be because of either

vanishing of this amplitude as described by mean field theories like BCS, or because

of phase fluctuations21 which render φ random. Therefore the superconducting

transition is governed by either or J, depending on whichever is lower. In presence

Synopsis 29

tunneling DOS showing

non-vanishing of the

penetration depth and

because of amplitude

going to zero. On the other hand, for strongly disordered samples (kFl <4) we observe

that J ≤ showing the dominance of phase fluctuations to drive the superconducting

transition.

of strongly disordered s-wave superconductor, NbN

As discussed in section 2.2, STS measurements give direct access to local

density of states. Spatial inhomogeneity can be tracked by acquiring spatially resolved

STS data. In this section we study the ground state superconducting properties of NbN

through spatial resolved STS measurements. For spatially resolved spectroscopy

4 6 8 10 12

-4

-2

0

2

4

0.5

1.0

1.5

10.6K

5.8K

3.1K

-4 -2 0 2 4

0.5

1.0

b

6.4K

4.7K

2.6K

G(V)/GN(V) in the form of Colormap for four samples with

increasing disorder. (b), (d), (f), (h) shows representative

tunneling spectra at different temperatures.

30 Synopsis

tunneling conductance was acquired at each location on 32×32 grid over an area of

200×200nm at the lowest temperature for films with various disorder levels. Fig. 6

shows the normalized tunneling spectra acquired at 500mK along line for films of

various disorder levels. We observe that with increasing disorder (1) Coherence peaks

becomes progressively diffused, (2) Zero bias conductance value (GN(0)) increases and

(3) superconducting spectra becomes highly inhomogeneous.

4.1 Coherence peak height as a measure of local order parameter (OP)

We first concentrate on the nature of individual tunneling spectra. Fig. 7 shows

two representative A-A corrected spectra recorded at 500mK at two different locations

on the sample with Tc = 2.9K. The two spectra show a common feature: a dip close to

V = 0 associated with superconducting energy gap, while they differ strongly in the

coherence peak heights.

The density of

T C =6.4K

Figure 6 Normalized tunneling spectra acquired at 500mK along a line of length 200

nm for four samples with Tc=6.4K, 3.5K, 2.9K, 1.65K. The linear slope from each

spectrum has been corrected for clarity.

-4 -2 0 2 4

0.6

0.8

1.0

1.2

0.6

0.8

1.0

Figure 7 Representative background corrected spectra at

500mK Tc ∼ 2.9K. h is the average of the coherence peak

heights at positive (h1) and negative bias (h2), calculated

with respect to line passing through high bias region(black

line). GN corresponds to the spatially averaged background

spectrum recorded at 8 K.

Synopsis 31

sharp coherence peaks at the edge of the gap, associated with the long-range phase

coherent superconducting state. This is quantitatively described by a single particle

DOS of the form23,

() = ( || + Γ

√(|| + Γ)2 − Δ2 ) (4)

broadening of the DOS due recombination of electron and hole-like quasiparticles. For

Cooper pairs without phase coherence, it is theoretically expected that the coherence

peaks will get suppressed whereas the gap will persist13. Therefore, we associate the

two kinds of spectra with regions with coherent and incoherent Cooper pairs

respectively7. The normalized tunneling spectra with well defined coherence peaks can

be fitted well within the BCS- formalism using eq. 1 and 3. Fig 8(a), 8(c) and 8(e)

show the representative fits for the three different samples. In all the samples we

observe to be dispersed between 0.8-1.0 meV corresponding to a mean value of

2/kBTc ~ 12.7, 7.2 and 6 (for Tc ~ 1.65 K, 2.9 K and 3.5 K respectively) which is much

larger than the value 3.52 expected from BCS theory19. Since is associated with the

0.6

0.8

1.0

0.6

0.8

1.0

0.4

0.8

1.2

0.4

0.8

1.2

0.4

0.8

1.2

0.4

0.8

V(mV)

Figure 8 Pairing energy and the onset of the soft gap in representative spectra for three

samples with Tc = 1.65K, 2.9K and 3.5K. (a), (c), (e) Normalized tunneling spectra (red)

on three different sample exhibiting well defined coherence peaks. Black curves

correspond to the BCS-Γ fits using the parameters shown in each panels. (b), (d), (f)

Normalized tunneling spectra at a different location on the same samples as shown in

(a)-(c) showing no coherence peaks; note that the onset of the soft gap in these spectra

coincide with the coherence peak positions in (a)-(c).

32 Synopsis

pairing energy scale, the abnormally large value of 2/kBTc and the insensitivity of

on Tc suggest that in the presence of strong disorder Tc is not determined by . On the

other hand, seems to be related to T* ~ 7-8 K which gives /kBT* ~ 3.00.2, closer to

the BCS estimate. is relatively large and shows a distinct increasing trend with

increase in disorder. In contrast, spectra that do not display coherence peaks (Fig. 8(b),

8(d) and 8(f)) cannot be fitted using BCS- form for DOS. However, we note that the

onset of the soft-gap in this kind of spectra happens at energies similar to the position

of the coherence peaks,showing that the pairing energy is not significantly different

between points with and without coherence.

Since the coherence peaks are directly associated with phase coherence of the

Cooper pairs, the height of the coherence peaks provides a direct measure of the local

superconducting order parameter. This is consistent with numerical Monte Carlo

simulations13 of disordered superconductors using attractive Hubbard model with

random on-site disorder which show that the coherence peak height in the LDOS is

directly related to the local superconducting OP Δ() = ⟨↓↑⟩. Consequently, we

take the average of the coherence peak height ( = ( + ) ⁄ ) at positive and

negative bias (with respect to the high bias background) as an experimental measure of

the local superconducting OP (Fig. 7(a)).

4.2 Emergence of inhomogeneity in the superconducting state

To explore the emergence of inhomogeneity we plot in Fig. 9(a), 9(b) and 9(c)

the spatial distribution of h, measured at 500 mK in the form of intensity plots for three

samples over 200 200 nm area. The plot shows large variation in h forming regions

where the OP is finite (yellow-red) dispersed in a matrix where the OP is very small or

completely suppressed (blue). The yellow-red regions form irregular shaped domains

dispersed in the blue regions. The fraction of the blue regions progressively increases

as disorder is increased. To analyse the spatial correlations we calculate the

autocorrelation function (ACF), defined as,

() = 1

(( − ) − ⟨⟩) (5)

where n in the total number of pixels and h is the standard deviation in h. The

circular average of x is plotted as a function of x in Fig. 9(j) showing that the

Synopsis 33

correlation length becomes longer as disorder is increased. The domain size

progressively decreases with decrease in disorder and eventually disappears in the noise

level for samples with Tc ≥ 6K. From the length at which the ACF drops to the levels

of the base line we estimate the domains sizes to be 50 nm, 30 nm and 20 nm for the

samples with Tc ~ 1.65 K, 2.9 K and 3.5K respectively. The emergent nature of the

superconducting domains is apparent when we compare structural inhomogeneity with

the h-maps. While the defects resulting from Nb vacancies are homogeneously

0 50 100 150 200 0.00

0.05

0.10

0.15

0.5

0.6

0.7

0.1

0.2

0.4

0.6

0.8

0.45

0.60

0.75

0.2

0.4

0.2

0.4

0.15

0.30

0.25

0.50

0.75

1.00

distance (nm)

C o

rr e

la ti

o n

Figure 9 (a)-(c) shows colormap of spatial evolution of h for sample with Tc = 1.65K,

2.9K and 3.5K respectively, (d)-(f) show the corresponding colormap of ZBC (GN(V=0))

and (g)-(i) show corresponding 2D histogram of h and ZBC. Weak anticorrelation

between h maps and ZBC maps can be seen from the two maps and it is further evident

from 2D histograms as we see the dense line with negative slope. The values of Tc

corresponding to each row for panels (a)-(i) are given on the left side of the figure. (j)

Radial average of the 2-dimensional autocorrelation function plotted as a function of

distance for the three samples.

34 Synopsis

distributed over atomic length scales, the domains formed by superconducting

correlations over this disordered landscape is 2 orders of magnitude larger.

The domain patterns observed in h-maps is also visible in Fig. 9(d), 9(e)

and 9(f) when we plot the maps of zero bias conductance (ZBC), GN(0), for the same

samples. The ZBC maps show an inverse correlation with the h-maps: Regions where

the superconducting OP is large have a smaller ZBC than places where the OP is

suppressed. The cross-correlation between the h-map and ZBC map can be computed

through the cross-correlator defined as,

= 1

,

(6)

where n is the total number of pixels and ZBC is the standard deviations in the

values of ZBC. A perfect correlation (anti-correlation) between the two images would

correspond to I = 1(-1). We obtain a cross correlation, I ≈ -0.3 showing that the anti-

correlation is weak. Thus ZBC is possibly not governed by the local OP alone. This is

also apparent in the 2-dimensional histograms of h and ZBC (Fig. 9(g), 9(h) and 9(i))

which show a large scatter over a negative slope.

4.3 Universal scaling of the order parameter distribution

In this section we analyse the statistical properties of OP. For quantitative

analysis we define the normalized local order parameter as,

=

[] (7)

Fig. 10(a) shows the order parameter (S) distribution (OPD) for four samples

with Tc = 1.65K, 2.9K and 3.5K and 6.4K. We observe that for the sample with Tc =

6.4K OPD peaks around S = 0.4. With increasing disorder this weight gradually shifts

towards zero and also the OPD gets widen. This is the indication of gradual formation

of regions where the superconducting OP is suppressed. We introduce the new scaling

variable,

(8)

where = exp (ln ) and 2 = ln2 S − ln 2. When plotted the probability

distribution for rescaled OP ( Fig. 10(b) ) we see that rescaled OPD for all the samples

Synopsis 35

universality of the OPD The OPD is

also in good agreement with Tracy-

Widom distribution whose relevance

finite dimensions24,25. We also

OPD within two prototype fermionic

and bosonic models for disordered

superconductors26 showing an

excellent agreement between

the local OP.

NbN

In this section we will focus on temperature evolution of domain structure that

is seen at the lowest temperature as the system is driven across Tc into pseudogap state.

At high temperatures coherence peaks get diffused due to thermal broadening and the

h-maps can no longer be used as a reliable measure of the OP distribution. This problem

is however overcome by tracking the zero bias conductance (ZBC) value in the

tunneling spectra to track temperature evolution of domains based on our observation

of weak anticorrelation between h maps and ZBC maps at lowest temperature.

We investigated the temperature evolution of the domains as a function of

temperature for the sample with Tc ~ 2.9 K. The bulk pseudogap temperature was first

determined for this sample by measuring the tunneling spectra at 64 points along a 200

nm line at ten different temperatures. Fig.11(a) shows the temperature evolution of the

normalized tunneling spectra along with temperature variation of resistance. In

0.0 0.2 0.4 0.6 0.8 0

1

2

3

0.2

0.4

0.6

6.4K

3.5K

2.9K

1.65K

TW

distribution for the four samples (b) The

same data as in panel (a) plotted in terms of

the rescaled variable RS. The solid line

corresponds to the Tracy-Widom

36 Synopsis

principle, at the T*, GN(V = 0) GN(V>>/e). Since this cross-over point is difficult to

uniquely determine within the noise levels of our measurements, we use GN(V = 0)/GN

(V = 3.5 mV) ~ 0.95 as a working definition for the T*. Using this definition we obtain

T* ~ 7.2 K for this sample.

Spectroscopic maps were subsequently obtained at 6 different temperatures

over the same area as the one in Fig. 9(e). Before acquiring the spectroscopic map we

0 50 100 150 200

0.3

0.4

0.5

0.6

0.3

0.4

0.5

0.6

0.7

0.3

0.4

0.5

0.6

0.7

0.4

0.6

0.8

0.6

0.8

1.0

0.6

0.8

1.0

Figure 11 Temperature evolution of the inhomogeneous superconducting state

for the sample with Tc = 2.9K. (a) Temperature evolution of spatially averaged

normalized tunneling spectra plotted in the form of intensity plot of GN(V) as a

function of bias voltage and temperature. Resistance vs temperature (R-T) for the same

sample is shown in white curve on the same plot. Pseudogap temperature T* ~ 7.2 K is

marked with the dotted black line on top of the plot. (b)-(g) Spatial variation of ZBC

(GN(V=0)) plotted in the form of intensity plot over the same area for six different

temperatures.

Synopsis 37

corrected for the small drift using the topographic image, such that the maps were taken

over the same area at every temperature. Fig. 11(b)-(g) show the ZBC maps as a

function of temperature. Below Tc, the domain pattern does not show a significant

change and for all points ( = 0) ( = 3.5)⁄ < 1 showing that a soft gap is

present everywhere. As the sample is heated across Tc Most of these domains continue

to survive at 3.6K across the superconducting transition. Barring few isolated points (

< 5% ) the soft gap in the spectrum persist even at this temperature. At 6.9K, which is

very close to T*, most of the domains have merged in the noise background, but the

remnant of few domains, originally associated with a region with high OP is still

visible. Thus the inhomogeneous superconducting state observed at low temperature

disappears at T*.

These observations provides a real space perspective on the formation of the

pseudogap state through phase disordering. Below Tc the coherent superconducting

domains get Josephson coupled giving rise to the global zero resistance state. With

increase in temperature thermal fluctuations cause this coupling to get weaker. At Tc

the weakest coupling is broken and the phase coherence between domains with finite

superconducting OP get lost. However, superconducting correlations within domains

continue to persist up to much higher temperature T* giving rise to the pseudogap state

in tunnelling measurement.

Chapter 5. Summary

In this chapter we discuss the implication of our results on the nature of the

superconducting transition. In a clean conventional superconductor the

superconducting transition, well described through BCS theory, is governed by a single

energy scale, which represent the pairing energy of the Cooper pairs. Consequently,

Tc is given by the temperature where This is indeed the case for NbN thin films

in the clean limit. On the other hand in the strong disorder limit, the persistence of the

gap in the single particle energy spectrum in the pseudogap state and the insensitivity

of on Tc conclusively establishes that is no longer the energy scale driving the

superconducting transition. Indeed, the formation of an inhomogeneous

superconducting state supports the notion that the superconducting state should be

visualized as a disordered network of superconducting islands where global phase

38 Synopsis

superconducting islands. Consequently at Tc, the phase coherence would get destroyed

through thermal phase fluctuations between the superconducting domains, while

coherent and incoherent Cooper pairs would continue to survive as evidenced from the

persistence of the domain structure and the soft gap in the tunneling spectrum at

temperatures above Tc. Finally, at T* we reach the energy scale set by the pairing energy

where the domain structure and the soft gap disappears.

These measurements connect naturally to direct measurements of the superfluid

phase stiffness (J) performed through low frequency penetration depth and high

frequency complex conductivity ( 'i” ) measurements on similar NbN

samples. Low frequency measurements8 reveal that in the same range of disorder where

the pseudogap appears ( Tc ≤ 6K), J(T 0) becomes a lower energy scale compared to

High frequency microwave measurements27 reveal that in the pseudogap regime

the superfluid stiffness becomes strongly frequency dependent. While at low

frequencies J ( ”) becomes zero close to Tc showing that the global phase

coherent state is destroyed, at higher frequencies J continues to remain finite up to a

higher temperature, which coincides with T* in the limit of very high frequencies. Since

at the probing length scale set by the electron diffusion length at microwave

frequencies27 is of the same order as the size of the domains observed in STS, finite J

at these frequencies implies that the phase stiffness continues to remains finite within

the individual phase coherent domains. Similar results were also obtained from the

microwave complex conductivity of strongly disordered InOx thin films28.

In summary, we have demonstrated the emergence of an inhomogeneous

superconducting state, consisting of domains made of phase coherent and incoherent

Cooper pairs in homogeneously disordered NbN thin films. The domains are observed

both in the local variation of coherence peak heights as well as in the ZBC which show

a weak inverse correlation with respect to each other. The origin of a finite ZBC at low

temperatures as well as this inverse correlation is not understood at present and should

form the basis for future theoretical investigations close to the SIT. However, the

persistence of these domains above Tc and subsequent disappearance only close to T*

provide a real space perspective on the nature of the superconducting transition, which

is expected to happen through thermal phase fluctuations between the phase coherent

Synopsis 39

domains, even when the pairing interaction remains finite. However, an understanding

of the explicit connection between this inhomogeneous state and percolative transport

for the temperature above and below Tc is currently incomplete29,30,31 and its

formulation would further enrich our understanding of the superconducting transition

in strongly disordered superconductors.

We finally summarize the evolution of various energy scales as a

function of disorder for NbN. Superfluid stiffness J was measured using two coil

mutual inductance technique and converted to temperature scale using J/kB. is

obtained using the BCS relation,

=

1.76 (9)

where Δ(0) is ground state superconducting energy gap obtained by fitting

tunneling spectra using DOS given by equation (4). It is instructive to note that in the

range of disorder

1

10

100

Figure 12 Phase diagram of for strongly disordered NbN

showing various temperature scales as a function of kFl. Tc is

obtained transport measurement. T* is pseudogap temperature,

J/kB is the superfluid stiffness converted into temperature scale.

is obtained from BCS relation for superconducting

transition temperature and ground state energy gap Δ(0).

40 Synopsis

Phys. Today 51 39 (1998)

3 Sambandamurthy G et al, Phys. Rev. Lett. 94 017003 (2005); Baturina T I et

al, Phys. Rev. Lett, 98 127003 (2007); Nguyen H Q et al, Phys. Rev. Lett.

103 157001 (2009)

4 M. D. Stewart Jr., A. Yin, J. M. Xu, and J. M. Valles Jr.

Science 318 1273 (2007)

5 R. Crane, N. P. Armitage, A. Johansson, G. Sambandamurthy, D. Shahar, and

G. Grüner

Phys. Rev. B 75 184530 (2007)

6 B. Sacépé, C. Chapelier, T. I. Baturina, V. M. Vinokur, M. R. Baklanov, and

M. Sanquer

Nat. Comm. 1 140 (2010)

7 B. Sacépé, T. Dubouchet, C. Chapelier, M. Sanquer, M. Ovadia, D. Shahar,

M. Feigel'man, and L. Ioffe

Nat. Phys. 7 239 (2011)

8 M. Mondal, A. Kamlapure, M. Chand, G. Saraswat, S. Kumar, J. Jesudasan,

L. Benfatto, V. Tripathi, and P. Raychaudhuri

Phys. Rev. Lett. 106 047001 (2011)

9 P. W. Anderson et al, Phys. Rev. B 28 117 (1983); A. M. Finkelstein, Phys. B

197 636 (1994)

11 A. Ghosal, M. Randeria, and N. Trivedi

Phys. Rev. Lett. 81 3940 (1998)

12 Y. Dubi, Y. Meir and Y. Avishai

Nature, 449 876 (2007)

13 K. Bouadim, Y. L. Loh, M. Randeria, and N. Trivedi

Synopsis 41

Nat. Phys. 7 884 (2011)

14 M. Mondal, M. Chand, A. Kamlapure, J. Jesudasan, V. C. Bagwe, S. Kumar,

G. Saraswat, V. Tripathi and P. Raychaudhuri, J. Supercond. Nov. Magn. 24

341 (2011)

15 S. P. Chockalingam, Madhavi Chand, John Jesudasan, Vikram Tripathi and

Pratap Raychaudhuri

Phys. Rev. B 77, 214503 (2008)

16 M. Chand, A. Mishra, Y. M. Xiong, A. Kamlapure, S. P. Chockalingam, J.

Jesudasan, V. Bagwe, M. Mondal, P. W. Adams, V. Tripathi, and P.

Raychaudhuri

Phys. Rev. B 80, 134514 (2009)

17 A. Kamlapure, T. Das, S. C. Ganguli, J. B Parmar, S. Bhattacharyya, P.

Raychaudhuri

arxiv.org/abs/1308.2880 (2013)

18 A. Kamlapure, G. Saraswat, S.C. Ganguli, V. Bagwe, P. Raychaudhuri, S. P

Pai

Mineola, New York, 2004).

Phys. Rev. Lett. 44 1288 (1980).

21 V. J. Emery and S. A. Kivelson,

Phys. Rev. Lett. 74 3253 (1995).

22 M. Chand, G. Saraswat, A. Kamlapure, M. Mondal, S. Kumar, J. Jesudasan,

V. Bagwe, L. Benfatto, V. Tripathi, and P. Raychaudhuri

Phys. Rev. B 85, 014508 (2012)

23 Dynes, R. C., Narayanamurti, V., and Garno, J. P. Direct Measurement of

Quasiparticle-Lifetime Broadening in a Strong-Coupled Superconductor. Phys.

Rev. Lett. 41, 1509 (1978).

24 C. Monthus and T. Garel, J. Stat. Mech.: Theory Exp. P01008 (2012)

25 C. Monthus and T. Garel, J. Phys. A: Math. Theor. 45, 095002 (2012).

26 G. Lemarié, A. Kamlapure, D. Bucheli, L. Benfatto, J. Lorenzana, G. Seibold,

S. C. Ganguli, P. Raychaudhuri and C. Castellani

42 Synopsis

Phys. Rev. B 85 184509 (2013)

27 M. Mondal, A. Kamlapure, S. C. Ganguli, J. Jesudasan, V. Bagwe, L.

Benfatto and P. Raychaudhuri.

Scientific Reports 3, 1357 (2013).

28 Liu, W., Kim, M., Sambandamurthy, G. and Armitage, N. P.

Phys. Rev. B 84, 024511(2011).

29 Bucheli, D., Caprara, S., Castellani, C. and Grilli, M.

New Journal of Physics 15, 023014 (2013).

30 Li, Y., Vicente, C. L. and Yoon, J.

Phys. Rev. B 81, 020505(R) (2010).

31 Seibold, G., Benfatto, L., Castellani, C. & Lorenzana, J.

Phys. Rev. Lett. 108, 207004 (2012).

Chapter 1

The phenomenon of superconductivity was discovered by Heike Kamerlingh

Onnes in 1911 where he observed a sudden drop to zero in the resistivity of Mercury,

to an experimental error, at 4.2K. Soon after, many more materials such as aluminium,

lead, tin etc. showed the superconductivity on cooling. The temperature below which

material turns superconducting is called as critical temperature (Tc). In 1933 it was

found by Walter Meissner and Robert Ochsenfeld that superconductor expels the weak

external applied magnetic field from entering into the bulk. The expulsion of magnetic

field would not take place in perfect conductor of free electrons, showing that the

superconductor is more than just perfect conductor.

Since the discovery of superconductivity, theorists struggled for several

decades to understand the origin of superconductivity although major advances made

through phenomenological theories mainly by London in 1935 and Ginzburg-Landau

Figure 1-1 Basic requirements of superconductivity: (a) Zero resistance state

below 4.2K as discovered by Kamerlingh Onnes in 1911, (b) Meissner- Ochsenfeld effect

showing expulsion of magnetic field below critical temperature

44 Chapter 1. Introduction

in 1950. It is John Bardeen, Leon Neil Cooper, and John Robert Schrieffer (BCS) who

first gave the microscopic theory of superconductivity in 1957. The basic idea in the

BCS theory is that in the superconducting state electrons pair though phonon coupling

and these pairs, called as Cooper pairs, condense into a single phase coherent ground

state which allows the electrons to move without scattering.

For the obvious technological reasons search for the new materials which could

superconduct at higher temperatures continued and in 1986 Alex Müller and Karl

Bednorz discovered a new class of superconductor known as the doped rare earth

cuprates. These materials become superconducting above 30K. In following years a

host of new material were found which superconduct at temperatures much higher than

the boiling point of liquid N2. These new class of materials are called as high

temperature superconductors (HTSC). Not much progress is made in understanding the

origin of HTSC although there are theories which qualitatively explain the possible

mechanism of pairing and symmetry of the gap.

While the quest for new materials continued, there have been also the

investigations by some researchers on the effect of disorder on superconducting

properties of the material. The problem gives a unique opportunity to study the

competition between superconductivity which results from pairing and the pair

breaking effects of electron localization and disorder induced Coulomb repulsion. The

interest in the field was further increased by the possibility that the disorder driven or

magnetic field driven suppression of superconductivity in the limit of zero temperature

might be a quantum phase transition.

In this thesis we study the effect of disorder on superconducting properties of

s-wave superconductor, NbN, close to metal insulator transition. The study was mainly

carried out using home built low temperature Scanning Tunneling Microscopes (STM).

The plan of the introduction chapter is as follows. In the first section I will describe the

basics of superconductivity and essential concept required to make platform for our

study. I will then review the experimental and theoretical advances in the field of

disorder/ magnetic field driven superconductor insulator transition (SIT). I will finally

introduce to our model system NbN and its characterization through transport

measurements and transmission electron microscopy (TEM).

Chapter 1. Introduction 45

1.1 Basics of Superconductivity

1.1.A The Meissner-Ochsenfeld effect

When a superconductor is cooled below its Tc and kept in a weak external

magnetic field then it expels the magnetic flux lines from entering into the bulk so that

the field inside a superconductor is zero (B = 0). This phenomenon is called as

Meissner-Ochsenfeld effect. Although superconductors show the perfect diamagnetism

at low fields, strong magnetic fields destroy the superconductivity. The field at which

superconductivity breaks down is called as the critical field (Bc)

1.1.B The London equations

The phenomenological theory developed by London brothers1 in 1935 explains

the perfect conductivity as well as the Meissner effect where they showed that the

superconductor produces screening current at the surface which shields the external

magnetic field from entering into the bulk. The two equation governing electromagnetic

fields inside a superconductor are,

= 2

The first equation essentially explains the perfect conductivity through the free

acceleration of charge. Using the identities in vector calculus and Amperes law one can

deduce the second equation to,

∇2 = 1

2 (1.3)

Where is called as London penetration depth and is defined as,

= √ 2

42 (1.4)

One can immediately see that on application of magnetic field = to

semi-infinite superconductor (Figure 1-2), the magnetic field inside the superconductor

is given by

46 Chapter 1. Introduction

Figure 1-2 The boundary between superconductor and magnetic field. Blue curve

inside the superconductor shows exponential fall characterized by London penetration

depth λL. Orange curve show the dependence of the current density with distance inside

the superconductor.

() = − ⁄ for x ≥ 0 (1.5)

i.e. the magnetic field inside the superconductor decreases exponentially and in

the bulk we find B → 0, hence the Meissner effect. Also from the second London

equation (Equ. 1.2) along with equation of continuity (∇ = 0) it follows that,

() = −

− ⁄ for x ≥ 0 (1.6)

Thus the supercurrents flow in the direction parallel to the surface and

perpendicular to B and decrease into the bulk over the same scale .

1.1.C Nonlocal Response: Pippard Coherence length ( ξ0 )

The nonlocal generalization of the London equations was proposed by Pippard2.

He argued that the superconducting wavefunction has a characteristic dimension ξ.

Superconducting properties such as superfluid density changes over the length scale of

ξ which can be estimated using uncertainty principle and is given by,

Chapter 1. Introduction 47

ξ =

(1.7)

Where α is a numeric constant of the order of unity. BCS theory predicts that

the value of α ≈ 0.18. It also has a physical significance in BCS theory that it represents

the size of the Cooper pairs.

1.1.D Ginzburg Landau (G-L) model of superconductivity

The phenomenological theory of superconductivity was introduced by

Ginzburg and Landau3 in 1950 which describes superconducting phase transition

within Landau’s general theory of second order phase transition. They introduced a

complex pseudo-wave function = || as an order parameter to describe

superconducting electrons.

G-L equation can be obtained using the variational principle to minimize the

free energy and it has the form analogous to Schrodinger’s equation,

1

= ∗

∗2

∗ ||2 (1.9)

With = || and using equ. 1.8 we can get the equation for supercurrent

velocity as,

=

2 (∇ −

) (1.10)

It can be shown that G-L order parameter can be related to local density of

superelectrons as,

Phase stiffness

Bulk superconducting ground state is described by a constant order parameter,

, where the phase of the order parameter, , has a constant value everywhere. There

is an energy cost associated with changing from one part of the superconductor to

another. This energy cost is called as phase stiffness or superfluid stiffness and denoted

as J. From equ. 1.10, the velocity of the superfluid is given by,

=

2 (∇φ) (1.12)

Now the increase in kinetic energy by phase twist is given by

∫ 3 (

4 ∫3(∇)2. In analogy with XY model4,5 in statistical

physics we define J over the cut-off distance as6,7,

= 2

4 (1.13)

For all our analysis we take the minimum cut-off distance a equal to coherence

length ξ as it is a characteristic length scale over which the superconducting parameters

changes. It is important to note that ∝ which is related to λL (equ. 1.4) which is

experimentally measureable quantity.

Solving G-L equation at the interface of superconductor introduces a

characteristic length called as G-L coherence length given by = ( 2

2∗|()| ) 1 2⁄

and it

is the measure of the distance over which order parameter respond to a perturbation.

To the first order approximation in α, it can be written as, () = (0)||−1 2⁄ , where

= −

= √ 2

82 (− ) (1.14)

Chapter 1. Introduction 49

The ratio =

is called as G-L parameter is an important parameter and is

independent of temperature within G-L theory.

Type I and Type II superconductors

The superconductors with G-L parameter < 1

√2 are called as Type-I

superconductors. These materials show a perfect diamagnetism at all fields below a

critical field Hc where the superconductivity is completely destroyed. Most elemental

superconductors are Type-I superconductors. In 1957 Abrikosov8 showed that for

superconductors with > 1

√2 , there exist an equilibrium state in presence of magnetic

field where the field lines penetrate the superconductors to form vortices. These

materials are called as Type-II superconductors. Vortices in Type-II superconductors

are formed above the lower critical field Hc1 and there is continuous increase in the flux

penetration till the upper critical field Hc2 where the superconductivity is completely

destroyed.

These vortices in Type-II superconductors form a triangular lattice9 and each

vortex contains exactly one quantum of flux, Φ0 = 2⁄ = 2.07 × 10−15 Wb. The

nearest neighbour distance for the vortex lattice is given by,

= 1.075 ( Φ0 ) 1 2⁄

(1.15)

Figure 1-3(a) shows the contour diagram for ||2in presence of magnetic field for

Figure 1-3 Abrikosov Flux lattice: (a) theoretically calculated contour diagram of

|| just below the upper critical field (b) triangular lattice of flux lines on the surface of

Pb. The black dots are cobalt particles.

50 Chapter 1. Introduction

type-II superconductor. Figure 1-3(b) shows the results of first experiment to visualize

the vortex lattice10.

Microscopic theory of superconductivity given by Bardeen, Cooper and

Schrieffer11 (BCS) in 1957 explains the superconductivity in many metals and predicts

many properties. The idea behind the theory is that ground state of free electrons is

unstable against the small attractive interaction between electrons12, no matter how

small is the interaction and the electrons pair to form bound state. The attractive

interaction between the electrons is provided by electron phonon exchange which can

be understood as follows: an electron with negative charge –e attracts the positively

charged ions as it moves in the crystal and the lattice distortion locally induces

excessive positive charge. This positive charge is in turn attracts another electron

forming a bound state with the first one. The cartoon picture showing the phonon

mediated attraction is as shown in Figure 1-4.

Figure 1-4. Cartoon picture of Cooper pair, pair of electrons with equal and

opposite momenta.

Cooper showed in that the bound state energy of the electron pair with equal

and opposite momenta and spin is given by,

ε = −2ω −(2 (0)⁄ ) (1.16)

Chapter 1. Introduction 51

where is the cut-off frequency corresponding to the Debye temperature. Next

we will briefly review the BCS theory11.

BCS took the form for the ground state as,

| = ∏ ( + ↑ + −↓

+ )|0

Where || 2 + ||

2 = 1 and |0 is the vacuum state. Coefficients and

are chosen so as to minimize the expectation value of the energy using the so called

reduced Hamiltonian,

−↓ + −↓↑ (1.17)

BCS assumed the simple form for the attractive interaction as,

= { −, |ξ|and |ξ| ≤ ω 0, Otherwise

(1.18)

Where ξ is the single particle energy of the electrons with respect to Fermi

energy. Following are the important key results of BCS theory,

The gap function

Δ(0) = 2ω −1 (0)⁄ (1.19)

Where Δ is the superconducting energy gap formed at the Fermi level and (0)

is Fermi level density of states.

Temperature dependence of the gap and Tc

Temperature dependence of the gap can be numerically calculated using,

1

(0) = ∫

(2 + Δ2)1 2⁄

ω

0

(1.20)

where = () −1. Figure 1-5 shows the temperature dependence of which

holds in good approximation for most of the conventional superconductors.

52 Chapter 1. Introduction

The critical temperature is the temperature at which Δ() → 0. Thus the integral

1.16 can be evaluated by substituting Δ = 0 and it yields,

= 1.13ω −1 (0)⁄ (1.21)

Comparing with Equ. 1.15 we get,

Δ(0) = 1.764 (1.22)

Figure 1-5. Temperature dependence of energy gap within BCS theory.

BCS density of states

The quasiparticles excitation energy within BCS theory is given by 2 =

2 + 2 which shows the minimum excitation to be i.e. there is a gap in the energy

spectrum. The single particle density of states (DOS) is given by,

()

Chapter 1. Introduction 53

Figure 1-6. Density of states in superconducting state compared to the normal

state.

1.1.F Electron tunneling and measurement of

In 1960 Giaever13 introduced a method to measure the for the superconductor

based on the principle of quantum mechanical tunneling. The measurements involves

tunnel junction which consists of a normal metal and a superconductor separated by

very thin insulating layer. The tunneling current between normal metal and a

superconductor is given by,

∞

−∞

(1.24)

Where 2() is the BCS density of states and f is the Fermi function. More

direct comparison between theory and experiments can be made through the tunneling

differential conductance,

(1.25)

It can be seen that as → 0 the tunneling conductance mimics the density

of states for the superconductors,

54 Chapter 1. Introduction

2(0) (1.26)

Figure 1-7(a) shows the tunneling differential conductance spectra plotted as a

function of V for the NbN-oxide-Ag tunnel junction at various temperatures14. Solid

lines shows the fits using BCS density of states (Equ. 1.18) with additional broadening

parameter Γ which takes into account the additional broadening due to finite lifetime

of the superconducting quasiparticles15.

() = ( || + Γ

√(|| + Γ)2 − Δ2 ) (1.27)

Figure 1-7(b) shows the temperature evolution of and Γ plotted along with

resistivity Vs temperature curve.

0.5

1.0

1.5

2.0

2.5

0.0

0.4

0.8

1.2

1.6

0.2

0.4

0.6

0.8

1.0

m

Figure 1-7. Tunneling measurements on NbN/oxide/Ag planar tunnel junction with Tc =

14.9K. (a) G(V)-V spectra at different temperatures along with the BCS-Γ fits, (b)

Temperature dependence of , Γ and ρ.

1.2 Disordered Superconductors

The interplay of superconductivity and disorder is one of the most intriguing

problems of quantum many body physics. Superconducting pairing interactions in a

normal metal drives the systems into a phase coherent state with zero electrical

resistance. In contrast, in a normal metal increasing disorder progressively increases

the resistance through disorder scattering eventually giving rise to an insulator at high

disorder where all electronic states are localized. Quite early on, it was argued by

Anderson16 that since BCS superconductors respect time reversal symmetry,

Chapter 1. Introduction 55

superconductivity is robust against nonmagnetic impurities and the critical temperature

Tc is not affected by such disorder. Anderson’s idea however applies only to weakly

disordered systems, with their extended electronic states. In presence of strong disorder

experiments showed that it reduces Tc and ultimately drives the system into an

insulator17,18,19,20. This suppression of superconductivity could be thickness

driven21,22,23, magnetic field driven24 or disorder driven25,26. Various other novel

phenomena are observed in the vicinity of superconductor insulator transition (SIT).

The two key observations are (i) persistence of finite superconducting correlations

above Tc through measurements of finite high J stiffness above Tc in amorphous InOx

films27,28, finite spectral gap at zero bias in the conductance spectra much above Tc in

scanning tunneling microscope (STM) experiments29,30,31 etc., and (ii) presence of

superconducting correlations/ Cooper pairing through the measurements of activated

temperature dependence of resistance on the insulating side32, the giant peak in the

magnetoresistance in thin films33,34,35, magnetic flux quantization in nano-honeycomb

patterned insulating thin films of Bi36, a more recent transport37,38 and tunneling

experiments39.

Although the complete theoretical understanding of the nature of SIT is lacking,

in recent times numerous theoretical and numerical advances have been made. It is

shown that in the intermediate disorder limit the effect of disorder is to decrease the

pairing amplitude40,41 through an increase in the electron-electron (e-e) Coulomb

repulsion which results in decrease in Tc. In presence of strong disorder experimental

observations are understood qualitatively through number of prototype models of

disordered superconductors which are based on either fermionic42,43,44,45,46 or

bosonic47,48,49 description. The fermionic models demonstrated the survival spectral

gap across SIT and the transition is driven by phase fluctuation between

superconducting islands. Bosonic models indicated that the SIT is driven by quantum

phase fluctuations between localized Cooper pairs.

In particular here I would like to highlight on the recent numerical simulations

which have direct relevance to the work presented in this thesis. These simulations

involve solving Attractive (negative-U) Hubbard model with random on-site

energy43,50,45. While these studies ignore Coulomb interactions and are done on

relatively small systems compared to real superconductors, they nevertheless support

56 Chapter 1. Introduction

key aspects of the basic scenario of the disordered superconductors namely (i) Single

particle spectral gap in the DOS at lowest temperature survives through SIT and is finite

everywhere though it is highly inhomogeneous. However J, decreases rapidly with

increasing disorder making the system more susceptible to phase fluctuations. (ii)

Coherence peak heights at the gap edge are directly correlated to the local

superconducting order and vanish with increasing temperature and disorder. (iii) Near

SIT, pseudogap appears in the DOS at low energies above Tc and also on the insulating

side. These results are indeed in good agreement with our results on disordered NbN

presented in this thesis.

In spite of the fact that the field of disordered superconductors has produced

variety of novel phenomena and interesting theoretical results which has enriched our

understanding of SIT to a great extent, more experimental works are needed for

complete understanding and resolving the open questions in the field. More

specifically, in regard of theoretical propositions, suggesting the emergence novel

phenomena beyond the ambit of BCS theory, there is very little direct experimental

evidence confirming the predictions made. In this thesis we address most of the

experimental remedies through our investigation on NbN which can be grown with

larger atomic defects by tweaking growth parameters.

1.3 Our model system: NbN

For our investigation we use NbN as a model system to study the effect of

disorder. NbN is a conventional s-wave superconductor with optimum Tc ~ 17K. Bulk

NbN has the λ of ~ 250 nm, electronic mean free of l ~ 4nm and the ξ ~ 5nm. It has

face centred cubic structure similar to NaCl. Band structure calculations show that

Fermi level lies within the 4d band and these electrons contribute to the conduction.

1.3.A Sample growth and introducing disorder

Epitaxial thin films of NbN are grown using reactive DC magnetron sputtering

in Ar+N2 gas mixture on (100) oriented single crystalline MgO substrate which is

heated to 600°C. The optimum conditions to get the highest Tc of 17K are sputtering

power =200W, Ar:N2 ratio = 84:16. The disorder in the system is tuned by varying

deposition conditions: either by decreasing the sputtering power keeping the partial gas

pressures constant or by increasing the N2 partial pressure51,52. In both these cases Nb

Chapter 1. Introduction 57

flux relative to N2 in the plasma is reduced which results in the Nb vacancies in the

crystal hence the disorder. For our study all the films are deposited with thickness ≥

50nm which is much larger than the dirty limit coherence length ~5-8 nm53 and can

be considered to be 3D as far as superconducting correlations are concerned.

1.3.B Structural characterization of NbN films

X-ray diffraction (XRD) study on films grown using above method show the

formation of crystalline NbN on MgO substrates54. All our films show high degree of

epitaxy as seen from the -scans using a four circle goniometer. This is further

confirmed directly through the high resolution transmission electron microscope

(HRTEM). Figure 1-8(a) and (b) show HRTEM images probed at the interface of

MgO

1 nm

Figure 1-8 TEM images (a), (b) High resolution TEM images for two samples

with Tc ~ 16K and 2.5K at the interface of NbN-MgO. (c), (d) corresponding high

resolution scanning TEM images.

substrate and NbN film along <110> direction for the two samples with Tc ~ 16K and

2.5K respectively. The difference between two samples at the atomic scale is revealed

58 Chapter 1. Introduction

in Figure 1-8(c) and (d) which shows the high resolution scanning transmission

(HRSTEM) images for same samples respectively. Intensity in the HRSTEM image is

primarily contributed by Nb and is proportional to the number of Nb atoms in the

probing column. Smooth intensity variation in clean sample (Tc ~ 16K) shows the

overall thickness variation produced during ion beam milling while the disordered

sample (Tc ~ 2.5K) shows random distribution of intensity in the columns showing

random number of Nb atoms in the adjacent columns. This clearly shows that for the

disordered films, the lattice contains Nb vacancies but when probed at the large scale

it is homogeneous. Thus we have an ideal system in which disorder is present at the

atomic length scale and the disorder is homogeneous over entire film.

1.3.C Quantification of disorder

To quantify disorder we use the Ioffe Regel parameter which is the measure

of mean free path in units of de-Broglie wavelength (). In clean system and

therefore has a large value. With increasing disorder decreases steadily due to

disorder scattering and therefore the quantity also decreases. At ≤ 1 all the

bloch states are completely localized which corresponds to Anderson metal insulator

transition (MIT). values are extracted from resistivity and Hall measurements and

calculated using free electron formula,

= (32)2 3⁄ [(285)]

1 3⁄

(285)5 3⁄ (1.28)

Here = − 1

assumes absence of e-e interaction which is not the case for

our disordered samples. Therefore we calculate at highest temperature of our

measurements (i.e. at 285K) where the effects of interaction is believed to be smaller55.

in our samples ranges from 10 (Tc = 16K) to all the way down to 0.42 (Tc < 300mK)

and we observe that ~ 1 is the critical disorder where superconductivity is

completely destroyed.

1.4 Effects of disorder

In this section we will review our recent work on disordered NbN through the

transport and λ measurements.

Chapter 1. Introduction 59

1.4.A Resistivity and measurement of Tc

Figure 1-9(a) shows resistivity Vs temperature curves ( − ) for full range of

disorder. The inset of Figure 1-9(a) shows the expanded view of − in the transition

region. Figure 1-9(b) shows the plot of Tc values with increasing disorder, Tc being the

temperature at which resistivity becomes 1% of its normal state value. Here we see that

→ 0 as → 0. Most disordered samples with < 1 do not show

superconducting downturn all the way down to 300mK. For these samples Tc is taken

as 300mK. From − curves we observe that except the least disordered sample with

= 10.12, all the samples show negative temperature coefficient which gets more

and more pronounced with increasing disorder.

50 100 150 200 250 300 10

-1

4

8

12

16

200

400

600

800

1000

0 2 4 6 8 10 12 14 16 18 20 10

-1

T (K)

Figure 1-9. (a) ρ – T for NbN films with different kFl, the inset shows the

expanded view in the transition region. (b) Variation of Tc with kFl, (c) Conductivity σ –

T at low temperature for the three samples with kFl = 0.82, 0.49 and 0.42. Extrapolations

to σ as → are shown with lines of different colour.

60 Chapter 1. Introduction

Figure1- 9(c) shows the conductivity Vs temperature − curves for three

most disordered samples with < 1. When extrapolated as → 0 the has finite

value which implies that our most disordered samples are not insulators but are bad

metals. Conventionally = 1 is associated with Anderson metal insulator transition.

The inconsistency between values and the observed metallic behaviour shows that

in presence of strong e-e interaction free electronic theory cannot be applied to measure

accurately values.

1.4.B Hall carrier density measurement

Carrier density (n) for the samples with various disorder is obtained by Hall

resistance measurement. Figure 1-10(a) shows plotted as a function of applied

magnetic field. Carrier density n is given by = −1 ⁄ where , the Hall

coefficient is extracted from the slope of − curves. Above relation for n is valid

only in the absence of e-e interactions therefore n is determined at 285K following

argument from section x. The measured carrier density for the stoichiometric NbN with

Tc ~ 16K is in good agreement with the band structure calculations56. Figure 1-10(b)

shows the n(285K) for films with increasing disorder.

0 4 8 12 -2.0

-1.5

-1.0

-0.5

0.0

5

10

15

20

25

0.49

0.82

1.68

3.27

5.5

k F l

Figure 1-10. Hall measurements, (a) ρxy – H measured at 285K for samples with

different kFl. (b) carrier density n extracted from ρxy and plotted as function of kFl.

Chapter 1. Introduction 61

1.4.C Upper critical field (Hc2) and coherence length (ξGL)

Figure 1-11 shows experimentally measured Hc2 and ξ for samples with varying

levels of disorder. We observe the non-monotonic behaviour in these quantities with

increasing disorder which can be

A Thesis

for the degree of Doctor of Philosophy

in Physics

Tata Institute of Fundamental Research

Mumbai

To my parents

This thesis is a presentation of my original research work.

Wherever contributions of others are involved, every effort is

made to indicate this clearly, with due reference to the literature,

and acknowledgement of collaborative research and discussions.

The work was done under the guidance of Professor Pratap

Raychaudhuri, at the Tata Institute of Fundamental Research,

Mumbai.

Anand Kamlapure

In my capacity as supervisor of the candidate’s thesis, I certify

that the above statements are true to the best of my knowledge.

Prof. Pratap Raychaudhuri

STATEMENT OF JOINT WORK

The experiments reported in this thesis have been carried out in the Department

of Condensed Matter Physics and Material Science under the guidance of Prof. Pratap

Raychaudhuri. The results of the major portions of the work presented in this thesis

have already been published in refereed journals.

Most of the experiments discussed in this thesis have been conducted by me in

the department. For completeness, I have included some of the experiments and data

analysis performed by other group members and collaborators.

Some of the scanning tunneling measurements were carried out jointly with

Garima Saraswat and Somesh Chandra Ganguli. Transport, Magnetoresistance and

Hall effect measurements were carried out in collaboration with Madhavi Chand.

Penetration depth measurements were carried out by Mintu Mondal and Sanjeev

Kumar. All the Transmission Electron Microscope measurements were carried out by

Tanmay Das and Somnath Bhattacharyya. Theoretical work was done in collaboration

with Dr. Vikram Tripathi of Department of Theoretical Physics, TIFR and Dr. Lara

Benfatto and Dr. Gabriel Lemarié of University of Rome, Rome, Italy.

PREFACE

The work presented in this thesis is on the experimental investigation of the

effect of disorder on s-wave superconductor NbN through scanning tunneling

spectroscopy (STS) measurements.

Disorder induced superconductor insulator transition (SIT) has been the subject

of interest since decades and there have been major advances both experimentally and

theoretically in understanding the nature of SIT. Recently new insights have been

offered by the numerical simulations which predicts unprecedented phenomena such

as persistence of gap across the SIT, spatial inhomogeneity in the gap and order

parameter, emergence of superconductivity over much larger length scale than the

disorder length scale, which needs to be addressed through sophisticated experiments.

The work presented in this thesis unravels many of these novel phenomena near the

SIT in s-wave superconductor, NbN, primarily through scanning tunneling

spectroscopy measurements and supported by results of penetration depth and transport

measurements.

The thesis is organized in following way, In Chapter 1, I will introduce the

motivation for our experiments on disordered superconductors through the advances in

the experimental and theoretical works. I will also introduce our model system: NbN

as a perfect system and its characterization through transmission electron microscope

at the atomic scale. In Chapter 2, I will elaborate on the basics of scanning tunneling

microscope (STM), fabrication of low temperature STM, related techniques and the

scheme of measurements. Chapter 3 focuses on our observation of formation of

pseudogap state in NbN in presence of strong disorder. We argue that the phase

fluctuation is the possible mechanism for the formation of pseudogap state. In Chapter

4, we investigate the ground state superconducting properties in strongly disordered

NbN through spatially resolved STS measurements. We identify that the coherence

peak height is a measure of local order parameter and show that the superconductivity

in the disordered NbN emerges over tens of nanometer scale while the structural

disorder present in the system is at atomic scale. In this chapter we also show that the

order parameter distribution in strongly disordered NbN has a universal behaviour

irrespective of the strength of disorder present in the system. We end the chapter with

the temperature evolution of inhomogeneous superconducting state through spatially

resolved STS measurements. In the concluding Chapter 5, I will summarize all our

investigation during past 6 years and present a phase diagram showing evolution of

various energy scales with disorder.

ACKNOWLEDGEMENTS

First and foremost, I would like to express my sincere gratitude to my thesis

advisor Prof. Pratap Raychaudhuri for the continuous support for my PhD work, for his

patience, motivation and enthusiasm.

I thank my fellow lab mates Garima Saraswat, Madhavi Chand, Mintu Mondal,

Sanjeev Kumar, Archana Mishra, Somesh Chandra Ganguli, Rini Ganguly, Harkirat

Singh, Prashant Shirage, John Jesudasan and Vivas Bagwe for their constant help and

support in every regard.

My sincere thanks goes to Subash Pai from Excel Instruments for all the prompt

technical support. I also thank Bhagyashree (Shilpa) Chalke, Rudhir Bapat, Nilesh

Kulkarni for the help in characterizing the samples and Atul Raut for technical help.

Most importantly I thank Low Temperature Facility team of TIFR for continuous

supply of liquid He and Nitrogen.

I also thank Vikram Tripathi, Lara Benfatto, Gabriel Lemarié for all the

discussions and theoretical support.

I take the opportunity to thank all my friends for their support, motivation and

all the fun we had during my Phd, especially I would like mention Sachin, Jaysurya,

Ajith, Gajendra, Abhishek, Nilesh, Harshad, Nikesh, Ashish, Amlan, Laskar, Bhanu,

Pranab, Abhishek, Mohon, Ronjoy, Sayanti, Anuj, Shishram, Vinod, Subhash, Amar,

Sunil, Abhijeet, Vinod, Jay, Jay, Sanjiv, Onkar, Shireen, Amul, Rajkiran, Lasse and

Pavel.

I finally thank my family members for their love and patience and I dedicate

this thesis to my parents.

LIST OF PUBLICATIONS

In refereed Journal and related to material presented here.

1. Emergence of nanoscale inhomogeneity in the superconducting state of a

homogeneously disordered conventional superconductor

Bhattacharya and Pratap Raychaudhuri

Scientific Reports 3 , 2979 (2013).

2. A 350 mK, 9 T scanning tunneling microscope for the study of superconducting

thin films and single crystals

Anand Kamlapure, Garima Saraswat, Somesh Chandra Ganguli, Vivas Bagwe,

Pratap Raychaudhuri and Subash P. Pai

Rev. Sci. Instrum. 84, 123905.

3. Universal scaling of the order-parameter distribution in strongly disordered

superconductors

G. Lemarié, A. Kamlapure, D. Bucheli, L. Benfatto, J. Lorenzana, G. Seibold, S.

C. Ganguli, P. Raychaudhuri and C. Castellani

Phys. Rev. B 87, 184509 (2013).

4. Phase diagram of the strongly disordered s-wave superconductor NbN close to the

metal-insulator transition

Madhavi Chand, Garima Saraswat, Anand Kamlapure, Mintu Mondal, Sanjeev

Kumar, John Jesudasan, Vivas Bagwe, Lara Benfatto, Vikram Tripathi, and Pratap

Raychaudhuri

Phys. Rev. B 85, 014508 (2012).

5. Phase Fluctuations in a Strongly Disordered s-Wave NbN Superconductor Close to

the Metal-Insulator Transition

Kumar, John Jesudasan, L. Benfatto, Vikram Tripathi, and Pratap Raychaudhuri

Phys. Rev. Lett. 106, 047001 (2011).

6. Enhancement of the finite-frequency superfluid response in the pseudogap regime

of strongly disordered superconducting films

Mintu Mondal, Anand Kamlapure, Somesh Chandra Ganguli, John Jesudasan,

Vivas Bagwe, Lara Benfatto and Pratap Raychaudhuri

Scientific Reports 3, 1357 (2013).

7. Temperature dependence of resistivity and Hall coefficient in strongly disordered

NbN thin films

Madhavi Chand, Archana Mishra, Y. M. Xiong, Anand Kamlapure, S. P.

Chockalingam, John Jesudasan, Vivas Bagwe, Mintu Mondal, P. W. Adams,

Vikram Tripathi, and Pratap Raychaudhuri

Phys. Rev. B 80, 134514 (2009).

8. Tunneling studies in a homogeneously disordered s-wave superconductor: NbN

S. P. Chockalingam, Madhavi Chand, Anand Kamlapure, John Jesudasan, Archana

Mishra, Vikram Tripathi, and Pratap Raychaudhuri

Phys. Rev. B 79, 094509 (2009).

In refereed journals, not related to the work presented

here.

1. Measurement of magnetic penetration depth and superconducting energy gap in

very thin epitaxial NbN films

Anand Kamlapure, Mintu Mondal, Madhavi Chand, Archana Mishra, John

Jesudasan, Vivas Bagwe, L. Benfatto, Vikram Tripathi, and Pratap Raychaudhuri

Appl. Phys. Lett. 96, 072509 (2010).

2. Andreev bound state and multiple energy gaps in the noncentrosymmetric

superconductor, BiPd

Mintu Mondal, Bhanu Joshi, Sanjeev Kumar, Anand Kamlapure, Somesh Chandra

Ganguli, Arumugam Thamizhavel, Sudhansu S. Mandal, Srinivasan Ramakrishnan

and Pratap Raychaudhuri

3. Role of the Vortex-Core Energy on the Berezinskii-Kosterlitz-Thouless Transition

in Thin Films of NbN

Mintu Mondal, Sanjeev Kumar, Madhavi Chand, Anand Kamlapure, Garima

Saraswat, G. Seibold, L. Benfatto, and Pratap Raychaudhuri

Phys. Rev. Lett. 107, 217003 (2011).

Conference Proceedings

1. Pseudogap state in strongly disordered conventional superconductor, NbN

Anand Kamlapure, Garima Saraswat, Madhavi Chand, Mintu Mondal, Sanjeev

Kumar, John Jesudasan, Vivas Bagwe, Lara Benfatto, Vikram Tripathi and Pratap

Raychaudhuri

J. Phys.: Conf. Ser. 400 022044 (2012).

2. Study of Pseudogap State in NbN using Scanning Tunneling Spectroscopy

Madhavi Chand, Anand Kamlapure, Garima Saraswat, Sanjeev Kumar, John

Jesudasan, Mintu Mondal, Vivas Bagwe, Vikram Tripathi, Pratap Raychaudhuri.

AIP Conference Proceedings 1349, 61.

3. Upper Critical Field and Coherence Length of Homogenously Disordered Epitaxial

3-Dimensional NbN Films

Kumar, Garima Saraswat, Vivas C Bagwe, Vikram Tripathi, Pratap Raychaudhuri

AIP Conference Proceedings 1349, 923.

4. Magnetoresistance studies of homogenously disordered 3-dimensional NbN thin

films

Saraswat, SP Chockalingam, John Jesudasan, Vivas Bagwe, Vikram Tripathi, Lara

Benfatto, Pratap Raychaudhuri

Films

Saraswat, Vivas C Bagwe, John Jesudasan, Lara Benfatto, Pratap Raychaudhuri

Journal of Physics: Conference Series 400 (2), 022078.

6. Effect of Phase Fluctuations on the Superconducting Properties of Strongly

Disordered 3D NbN Thin Films

Madhavi Chand, Mintu Mondal, Anand Kamlapure, Garima Saraswat, Archana

Mishra, John Jesudasan, Vivas C Bagwe, Sanjeev Kumar, Vikram Tripathi, Lara

Benfatto, Pratap Raychaudhuri

TABLE OF CONTENTS

1.1.C Nonlocal Response: Pippard Coherence length ( ξ0 ) ............... 46

1.1.D Ginzburg Landau (G-L) model of superconductivity ................ 47

Phase stiffness ............................................................................ 48

Type I and Type II superconductors .......................................... 49

1.1.E BCS theory of superconductivity ........................................................ 50

The gap function ........................................................................ 51

BCS density of states .................................................................. 52

1.1.F Electron tunneling and measurement of .................................... 53

1.2 Disordered Superconductors ........................................................................ 54

1.3.A Sample growth and introducing disorder...................................... 56

1.3.B Structural characterization of NbN films ....................................... 57

1.3.C Quantification of disorder ...................................................................... 58

1.4 Effects of disorder .............................................................................................. 58

1.4.A Resistivity and measurement of Tc.................................................... 59

1.4.B Hall carrier density measurement ..................................................... 60

1.4.C Upper critical field (Hc2) and coherence length (ξGL) ................ 61

1.4.D Magnetic penetration depth (λ).......................................................... 61

2.2 STM Theory ............................................................................................................71

2.3.A STM Head .......................................................................................................78

Coarse positioner: ...................................................................... 78

Piezoelectric tube ...................................................................... 80

Calibration of Piezo constants ................................................... 83

Tip preparation .......................................................................... 84

2.3.B Sample holder ..............................................................................................85

2.3.E 3He Cryostat ..................................................................................................89

Vibrational noise ........................................................................ 91

Electrical noise ........................................................................... 93

Normal Superconductor tunneling ............................................ 97

Conductance map ...................................................................... 99

2.5 Reference ............................................................................................................. 101

Chapter 3 ........................................................................................... 106

3.1.A In-situ preparation of NbN films ...................................................... 107

3.1.B Line scan and averaged spectrum .................................................. 108

3.1.C DOS evolution with temperature .................................................... 109

3.1.D Background correction for disorder NbN samples ................ 109

3.2 Experimental results ...................................................................................... 111

Regime III Nonsuperconducting regime ................................... 119

3.4 Summary .............................................................................................................. 120

3.5 References ........................................................................................................... 121

Chapter 4 .......................................................................................... 125

4.1 Introduction ....................................................................................................... 125

4.2 Investigation of structural disorder in NbN at the atomic scale.

......................................................................................................................................................... 126

......................................................................................................................................................... 129

4.5 Coherence peak height as a measure of local order parameter 130

4.6 Emergence of inhomogeneity in the superconducting state ...... 133

4.7 Universal scaling of the order parameter distribution .................. 135

4.8 Temperature evolution of the inhomogeneous superconduct .. 137

4.9 Discussion ............................................................................................................ 141

4.10 Summary ........................................................................................................... 142

4.11 References ........................................................................................................ 144

Chapter 5 .......................................................................................... 147

a lattice constant or characteristic length scale of phase fluctuations

e electronic charge

EF Fermi energy

Hc2 upper critical field

J superfluid stiffness

kB Boltzmann constant

kF Fermi wave-number

Mαβ Tunneling matrix element between the states α and β

n number density/ electronic carrier density

ns superfluid density

R resistance

resistivity

DOS density of states

HRTEM high resolution transmission electron microscope

HTSC high temperature superconductors

IVC inner vacuum chamber

MIT metal-insulator transition

Chapter 1. Introduction:

The interplay of superconductivity and disorder is one of the most intriguing problems

of quantum many body physics. Superconducting pairing interactions in a normal metal

drives the system into a phase coherent state with zero electrical resistance. In contrast,

in a normal metal increasing disorder progressively increases the resistance through

disorder scattering eventually giving rise to an insulator at high disorder where all

electronic states are localized. Quite early on, it was argued by Anderson1 that since

BCS superconductors respect time reversal symmetry, superconductivity is robust

against nonmagnetic impurities and the critical temperature Tc is not affected by such

disorder. However experiments showed that strong disorder reduces Tc and ultimately

drives the system into an insulator2. Various other phenomena are observed in the

vicinity of Superconductor Insulator transition (SIT) which includes the giant peak in

the magnetoresistance in thin films3, magnetic flux quantization in nano-honeycomb

patterned insulating thin films of Bi4, finite high frequency superfluid stiffness above

Tc in amorphous InOx films5, finite spectral gap in the conductance spectra much above

Tc in scanning tunneling microscope (STM) experiments6,7,8 etc. All of these points

towards the existence of finite superconducting correlation persisting in the system

even though the global superconductivity is destroyed due to disorder.

In recent times numerous theories and numerical simulations have been carried

out in order to understand the real space evolution of superconductivity in presence of

strong disorder. In the intermediate disorder limit the effect of disorder is to decrease

the pairing amplitude9 through an increase in the electron-electron Coulomb repulsion

which results in decrease in Tc. On the insulating side of SIT, it has been argued that

Cooper pair exists even after the single electrons states are completely localized10. The

numerical simulations involve solving Attractive Hubbard model with random on-site

energy11,12,13. Although these simulations ignore the Coulomb interactions and are done

on relatively small lattice the end results are instructive. These simulations indicate that

in the presence of strong disorder the superconducting order parameter becomes

inhomogeneous, spontaneously segregating into superconducting domains, dispersed

in an insulating matrix. Consequently the energy gap, Δ, is not strongly affected but the

energy cost of spatially twisting the phase of the condensate, superfluid stiffness J,

22 Synopsis

decreases rapidly with increasing disorder making the system more susceptible to phase

fluctuations. Thus, in presence of strong disorder near SIT, system consists of

superconducting islands and their phases are Josephson coupled through insulating

regions. Another interesting consequence of these simulations is that in presence of

strong disorder with lowering temperature, Copper pairs are formed above the Tc but

they are phase incoherent. Therefore one expects a resistive state but finite gap due to

superconducting correlations in the local density of states. This gap is termed as

pseudogap which resembles well established pseudogap in high Tc Cuprates.

1.1 Our model system: NbN

For our investigation we use thin films of NbN as a model for the study of effect

of disorder which can be grown by sputtering Nb in Ar + N2 gas mixture. NbN is s-

wave superconductor with relatively high Tc ~16K. Films are grown on single

crystalline MgO substrates and are highly epitaxial. All the films grown for the study

have thickness > 50nm which is much larger than the dirty limit coherence length x~5-

8 nm14 and can be considered to be 3D as far as superconducting correlations are

concerned. Disorder in the film can be tuned by varying the deposition conditions:

either by decreasing the sputtering power or by increasing N2 in the gas mixture15,16.

Disorder in the samples is characterized by Ioffe-Regel parameter, kFl, using the

formula

(1)

where RH is the Hall resistance and ρ is the resistivity, both of which are

measured using transport measurements. While our most ordered sample shows Tc

~16K, with increasing disorder Tc monotonically decreases all the way down to

<300mK. The range of kFl varies from 1 to 10.2 in our samples.

1.2 Structural characterization of disorder

Thin films of NbN grown using sputtering method show high degree of epitaxy

revealed through transmission electron microscopy (TEM) images17. Fig.1 (a) and (d)

show high resolution TEM images probed at the interface of MgO substrate and NbN

film along <110> direction for the two samples with Tc = 16K and 2.5K respectively.

Synopsis 23

The difference between the two films becomes prominent when we take high

resolution scanning TEM data (HRSTEM) as shown in Fig. 1. Panels (b) and (e) shows

HRSTEM image for the two samples with Tc = 16K and 2.5K and panels (c) and (f)

show corresponding two dimensional intensity distribution plots. Intensity in the

HRSTEM image is primarily contributed by Nb and is proportional to the number of

Nb atoms in the probing column. Smooth intensity variation in clean sample (Tc = 16K)

shows the overall thickness variation produced during ion beam milling while the

disordered sample (Tc = 2.5K) shows random distribution of intensity in the columns

showing random number of Nb atoms in the adjacent columns. This clearly shows that

for the disordered films, the lattice contains Nb vacancies but when probed at the large

scale it is homogeneous. Thus we have an ideal system in which disorder is present at

the atomic length scale and the disorder is homogeneous over entire film.

All the work presented in this thesis on disordered NbN is primarily carried out

in our home built STM. Details of the STM and measurement techniques are discussed

in the next chapter.

K

Figure 1 TEM images (a), (d) High resolution TEM images for samples with Tc = 16K and

2.5K respectively. (b), (e) corresponding high resolution scanning TEM images. (c), (f)

surface plots of 2 dimensional intensity distributions corresponding to (b) and (e)

respectively.

Chapter 2. Scanning tunneling microscope

Scanning tunneling microscope (STM) is a powerful tool to probe the electronic

structure of the material at the atomic scale. It works on the principle of quantum

mechanical tunneling between two electrodes through vacuum as a barrier. Essential

parts consist of a sharp metallic tip which is brought near the sample using positioning

units. Small bias applied between tip and sample make the tunneling current flow

between them which is amplified and recorded. Tunneling current exponentially

depends on the distance between tip and sample. By keeping the current constant,

distance between the tip and sample is held constant using feedback loop and by

scanning over the sample the topographic image of the sample is generated.

2.1 Setup

The overall schematic of our system is shown in Fig. 2(a). The assembly

primarily consists of three units, Sample preparation chamber, load lock and the 4He

dewar18. Sample preparation chamber comprises of two magnetron sputtering guns, two

Figure 2 (a) Schematic view of the home built low temperature scanning tunneling

microscope. Cryostat and magnet have been made semi-transparent to show the

internal construction. (b) Schematic view of the STM head shown along with the sample

holder.

Synopsis 25

evaporation sources, a plasma ion etching gun and a heater to heat the sample during

the deposition. Load lock chamber serves as the stage to transfer sample from

deposition chamber into the STM chamber using a pair of transfer manipulators. 4He

dewar has a 9T magnet which houses 3He insert. Helium cryostat hangs from custom

designed vibration isolation table mounted on pneumatic legs and consists of variable

temperature insert (VTI) and STM head. STM head (Fig. 2(b)) attached to the VTI

consists of sample housing assembly, positioning unit and printed circuit board for the

electrical connections. A combination of active and passive vibration isolation systems

are used to obtain the required mechanical stability of the tip. The entire system

operates in a high vacuum of 10-7 mbar and the base temperature for the measurements

is 350mK. Commercially bought control electronics and data acquisition unit (R9,

RHK Technology) is used carry out our experiments.

2.2 Methods

Thin films are grown on substrate mounted on specially designed sample holder

made of Molybdenum. The Molybdenum holder has threading on side and bottom for

holding on the manipulators. Substrate is secured in place on the holder using a cap

which also provides electrical contact with the sample for STM measurements. To

ensure electrical contact between film and holder (Fig. 3) substrate is pre-deposited

with NbN strips in another chamber and the actual film is grown on this strip in STM

chamber. Once the film is grown the

sample holder attached on

horizontal manipulator is pulled

with the vertical manipulator. Using

vertical manipulator the sample

temperature radiation coming from

of set of metal discs mounted on

steel rod is inserted in the annular

Figure 3 Design of sample holder (a)

Molybdenum cap, (b) Substrate with strip

deposited at the edge, (c) Molybdenum sample

holder, (d) Sample holder assembly, showing

substrate fastened with cap. (e) Resulting film

on the substrate after the deposition.

26 Synopsis

region of VTI. Once all the measurements are completed on the sample it is taken out

from the STM and resistivity versus temperature is measured in different cryostat.

2.3 Scanning tunneling spectroscopy

Another powerful technique using STM is to measure local density of states

through tunneling conductance measurements and the method is called as scanning

tunneling spectroscopy (STS). The tunneling conductance (G(V)) between the normal

metal tip and the superconductor is given by19,

() ∝ 1

∫ () (−

( − )

(2)

It can be shown that at sufficiently low temperatures Fermi function becomes

step function and () ∝ () i.e. the tunneling conductance is proportional to the

local density of states of the sample at energy E = eV. To measure the tunneling

conductance, tip sample distance is fixed by switching off the feedback loop and a small

alternating voltage is modulated on the bias. The resultant amplitude of the current

modulation as read by the lock-in amplifier is proportional to the / as can be seen

by Taylor expansion of the current,

( + sin()) ≈ () +

| . sin() (3)

The modulation voltage used in the measurement is = 150 and the

frequency used is 419.3Hz.

Temperature evolution of tunneling density of states (DOS) is investigated

through STS measurements along a line. Averaged spectra at different temperatures are

obtained by taking the average of about 20 spectra each at 32 equidistant points over

the line of length 200 nm and then averaging all in once. The ground state

superconducting properties and its temperature evolution are measured through

spatially resolved STS data. To acquire such data initially topography is imaged at

lowest temperature and then by defining a grid of 32×32 STS data is acquired at each

location (typically 5 spectra at each pixel and then averaged). For higher temperatures

we match the topography before acquiring spatially resolved STS data.

Synopsis 27

NbN

One of the most curious and debated state is the pseudogap state observed in

high Tc superconductors where finite gap in the DOS at Fermi level is observed much

above the superconducting transition temperature which evolves continuously from the

superconducting energy gap below Tc. Several scenarios based either on peculiarities

specific to High Tc Cuprates such as an order competing with superconductivity, or a

superconducting transition driven by phase fluctuations have been suggested as

possible origin of this feature. In this section we elucidate formation of pseudogap state

in NbN using scanning tunneling spectroscopy.

In strong disorder limit all the samples show two distinct features in tunneling

spectra: A low bias dip close to Fermi level which is associated with superconductivity

and a weakly temperature dependent V-shaped background which extends up to high

bias. This second feature which persists up to the highest temperature of our

measurements arises from the Altshuler-Aronov (A-A) type e-e interactions in the

normal state20. To extract the superconducting information from this data we divide the

low temperature spectra by the spectra at sufficiently high temperature where we do

not have any soft gap due to superconducting correlations. The temperature up to which

the pseudogap persists is defined as T*.

-3 -2 -1 0 1 2 3

0.7

0.8

0.9

1.0

4.4K

4.04K

3.61K

3.3K

3.1K

2.6K

0.8

0.9

-1.5

0.0

1.5

3.0

T*

V (

-100

0

100

3.1K

3.3K

3.61K

4.04K

5.33K

7K

9.35K

9.35K

8K

7K

6.28K

5.33K

4.84K

d v

V (mV)

Figure 4 (a) Normalized conductance curves for the sample with Tc=2.6K.

(b) Derivatives of the conductance curves in panel (a). Few curves are

removed for clarity. (c) Normalized conductance curves after dividing

curves in panel (a) from 9.35K data. (d) Surface plot of the curves of panel

(c)

28 Synopsis

Representative data for one of the strongly disordered samples (Tc = 2.6K) is

shown in Fig. 4. Fig. 4(a) shows conductance spectra at different temperatures. We

observe that the low bias gap feature disappears above 8K and the spectrum at 9.35K

has only the broad background. This is clearly seen in the dG(V)/dV versus V curves

(Fig. 4(b)) where the symmetric peak-dip structure associated with the low bias feature

completely disappears for the spectrum at 9.35K. Therefore to remove the A-A

background from the low temperature spectra we divide the spectrum at 9.35K. Fig.4(c)

shows the divided spectra and Fig. 4 (d) shows the colormap of divided data with x-

axis as the temperature, y-axis as the bias and the colorscale as the normalized

conductance value. The data in panel (d) shows that the pseudogap persists up to 6.5K

i.e. T* = 6.5K.

Series of NbN films with increasing disorder were studied using STS. Fig. 5

shows the temperature evolution of tunneling DOS for four samples with Tc = 11.9K,

6K, 2.9K and 1.65K in the form of colormap. All the plots in this figure are corrected

for Altshuler-Aronov background. R-T data for the same sample is indicated by thick

line on top of each colormap. Representative spectra at three temperatures are shown

to the right for clarity. Panel (a) Tc = 11.9K, shows that at low temperature spectra

consist of dip close to zero bias and two symmetric peaks consistent with BCS density

of states. The gap in the spectra vanishes exactly at Tc in accordance with BCS theory

and flat metallic DOS is restored for T > Tc. For the sample with Tc = 6K the gap

remains finite upto slightly higher temperature. For strongly disordered samples (Tc =

2.9K and 1.65K) the gap in the electronic spectra at the Fermi level persists all the way

upto ~7K showing that it forms the pseudogap state and the corresponding T*~ 7K.

Thus we observe that in presence of weak disorder gap closes exactly at Tc while for

strong disorder NbN forms a pseudogapped state above Tc.

Observation of pseudogapped state can be explained using phase fluctuation

scenario. Superconducting order is characterized by complex order parameter given by

Δ0eiφ, where Δ0 is amplitude of the order parameter (which is proportional to the

superconducting energy gap) and φ is the phase, which is same for the entire sample in

the superconducting state. The loss of superconductivity can be because of either

vanishing of this amplitude as described by mean field theories like BCS, or because

of phase fluctuations21 which render φ random. Therefore the superconducting

transition is governed by either or J, depending on whichever is lower. In presence

Synopsis 29

tunneling DOS showing

non-vanishing of the

penetration depth and

because of amplitude

going to zero. On the other hand, for strongly disordered samples (kFl <4) we observe

that J ≤ showing the dominance of phase fluctuations to drive the superconducting

transition.

of strongly disordered s-wave superconductor, NbN

As discussed in section 2.2, STS measurements give direct access to local

density of states. Spatial inhomogeneity can be tracked by acquiring spatially resolved

STS data. In this section we study the ground state superconducting properties of NbN

through spatial resolved STS measurements. For spatially resolved spectroscopy

4 6 8 10 12

-4

-2

0

2

4

0.5

1.0

1.5

10.6K

5.8K

3.1K

-4 -2 0 2 4

0.5

1.0

b

6.4K

4.7K

2.6K

G(V)/GN(V) in the form of Colormap for four samples with

increasing disorder. (b), (d), (f), (h) shows representative

tunneling spectra at different temperatures.

30 Synopsis

tunneling conductance was acquired at each location on 32×32 grid over an area of

200×200nm at the lowest temperature for films with various disorder levels. Fig. 6

shows the normalized tunneling spectra acquired at 500mK along line for films of

various disorder levels. We observe that with increasing disorder (1) Coherence peaks

becomes progressively diffused, (2) Zero bias conductance value (GN(0)) increases and

(3) superconducting spectra becomes highly inhomogeneous.

4.1 Coherence peak height as a measure of local order parameter (OP)

We first concentrate on the nature of individual tunneling spectra. Fig. 7 shows

two representative A-A corrected spectra recorded at 500mK at two different locations

on the sample with Tc = 2.9K. The two spectra show a common feature: a dip close to

V = 0 associated with superconducting energy gap, while they differ strongly in the

coherence peak heights.

The density of

T C =6.4K

Figure 6 Normalized tunneling spectra acquired at 500mK along a line of length 200

nm for four samples with Tc=6.4K, 3.5K, 2.9K, 1.65K. The linear slope from each

spectrum has been corrected for clarity.

-4 -2 0 2 4

0.6

0.8

1.0

1.2

0.6

0.8

1.0

Figure 7 Representative background corrected spectra at

500mK Tc ∼ 2.9K. h is the average of the coherence peak

heights at positive (h1) and negative bias (h2), calculated

with respect to line passing through high bias region(black

line). GN corresponds to the spatially averaged background

spectrum recorded at 8 K.

Synopsis 31

sharp coherence peaks at the edge of the gap, associated with the long-range phase

coherent superconducting state. This is quantitatively described by a single particle

DOS of the form23,

() = ( || + Γ

√(|| + Γ)2 − Δ2 ) (4)

broadening of the DOS due recombination of electron and hole-like quasiparticles. For

Cooper pairs without phase coherence, it is theoretically expected that the coherence

peaks will get suppressed whereas the gap will persist13. Therefore, we associate the

two kinds of spectra with regions with coherent and incoherent Cooper pairs

respectively7. The normalized tunneling spectra with well defined coherence peaks can

be fitted well within the BCS- formalism using eq. 1 and 3. Fig 8(a), 8(c) and 8(e)

show the representative fits for the three different samples. In all the samples we

observe to be dispersed between 0.8-1.0 meV corresponding to a mean value of

2/kBTc ~ 12.7, 7.2 and 6 (for Tc ~ 1.65 K, 2.9 K and 3.5 K respectively) which is much

larger than the value 3.52 expected from BCS theory19. Since is associated with the

0.6

0.8

1.0

0.6

0.8

1.0

0.4

0.8

1.2

0.4

0.8

1.2

0.4

0.8

1.2

0.4

0.8

V(mV)

Figure 8 Pairing energy and the onset of the soft gap in representative spectra for three

samples with Tc = 1.65K, 2.9K and 3.5K. (a), (c), (e) Normalized tunneling spectra (red)

on three different sample exhibiting well defined coherence peaks. Black curves

correspond to the BCS-Γ fits using the parameters shown in each panels. (b), (d), (f)

Normalized tunneling spectra at a different location on the same samples as shown in

(a)-(c) showing no coherence peaks; note that the onset of the soft gap in these spectra

coincide with the coherence peak positions in (a)-(c).

32 Synopsis

pairing energy scale, the abnormally large value of 2/kBTc and the insensitivity of

on Tc suggest that in the presence of strong disorder Tc is not determined by . On the

other hand, seems to be related to T* ~ 7-8 K which gives /kBT* ~ 3.00.2, closer to

the BCS estimate. is relatively large and shows a distinct increasing trend with

increase in disorder. In contrast, spectra that do not display coherence peaks (Fig. 8(b),

8(d) and 8(f)) cannot be fitted using BCS- form for DOS. However, we note that the

onset of the soft-gap in this kind of spectra happens at energies similar to the position

of the coherence peaks,showing that the pairing energy is not significantly different

between points with and without coherence.

Since the coherence peaks are directly associated with phase coherence of the

Cooper pairs, the height of the coherence peaks provides a direct measure of the local

superconducting order parameter. This is consistent with numerical Monte Carlo

simulations13 of disordered superconductors using attractive Hubbard model with

random on-site disorder which show that the coherence peak height in the LDOS is

directly related to the local superconducting OP Δ() = ⟨↓↑⟩. Consequently, we

take the average of the coherence peak height ( = ( + ) ⁄ ) at positive and

negative bias (with respect to the high bias background) as an experimental measure of

the local superconducting OP (Fig. 7(a)).

4.2 Emergence of inhomogeneity in the superconducting state

To explore the emergence of inhomogeneity we plot in Fig. 9(a), 9(b) and 9(c)

the spatial distribution of h, measured at 500 mK in the form of intensity plots for three

samples over 200 200 nm area. The plot shows large variation in h forming regions

where the OP is finite (yellow-red) dispersed in a matrix where the OP is very small or

completely suppressed (blue). The yellow-red regions form irregular shaped domains

dispersed in the blue regions. The fraction of the blue regions progressively increases

as disorder is increased. To analyse the spatial correlations we calculate the

autocorrelation function (ACF), defined as,

() = 1

(( − ) − ⟨⟩) (5)

where n in the total number of pixels and h is the standard deviation in h. The

circular average of x is plotted as a function of x in Fig. 9(j) showing that the

Synopsis 33

correlation length becomes longer as disorder is increased. The domain size

progressively decreases with decrease in disorder and eventually disappears in the noise

level for samples with Tc ≥ 6K. From the length at which the ACF drops to the levels

of the base line we estimate the domains sizes to be 50 nm, 30 nm and 20 nm for the

samples with Tc ~ 1.65 K, 2.9 K and 3.5K respectively. The emergent nature of the

superconducting domains is apparent when we compare structural inhomogeneity with

the h-maps. While the defects resulting from Nb vacancies are homogeneously

0 50 100 150 200 0.00

0.05

0.10

0.15

0.5

0.6

0.7

0.1

0.2

0.4

0.6

0.8

0.45

0.60

0.75

0.2

0.4

0.2

0.4

0.15

0.30

0.25

0.50

0.75

1.00

distance (nm)

C o

rr e

la ti

o n

Figure 9 (a)-(c) shows colormap of spatial evolution of h for sample with Tc = 1.65K,

2.9K and 3.5K respectively, (d)-(f) show the corresponding colormap of ZBC (GN(V=0))

and (g)-(i) show corresponding 2D histogram of h and ZBC. Weak anticorrelation

between h maps and ZBC maps can be seen from the two maps and it is further evident

from 2D histograms as we see the dense line with negative slope. The values of Tc

corresponding to each row for panels (a)-(i) are given on the left side of the figure. (j)

Radial average of the 2-dimensional autocorrelation function plotted as a function of

distance for the three samples.

34 Synopsis

distributed over atomic length scales, the domains formed by superconducting

correlations over this disordered landscape is 2 orders of magnitude larger.

The domain patterns observed in h-maps is also visible in Fig. 9(d), 9(e)

and 9(f) when we plot the maps of zero bias conductance (ZBC), GN(0), for the same

samples. The ZBC maps show an inverse correlation with the h-maps: Regions where

the superconducting OP is large have a smaller ZBC than places where the OP is

suppressed. The cross-correlation between the h-map and ZBC map can be computed

through the cross-correlator defined as,

= 1

,

(6)

where n is the total number of pixels and ZBC is the standard deviations in the

values of ZBC. A perfect correlation (anti-correlation) between the two images would

correspond to I = 1(-1). We obtain a cross correlation, I ≈ -0.3 showing that the anti-

correlation is weak. Thus ZBC is possibly not governed by the local OP alone. This is

also apparent in the 2-dimensional histograms of h and ZBC (Fig. 9(g), 9(h) and 9(i))

which show a large scatter over a negative slope.

4.3 Universal scaling of the order parameter distribution

In this section we analyse the statistical properties of OP. For quantitative

analysis we define the normalized local order parameter as,

=

[] (7)

Fig. 10(a) shows the order parameter (S) distribution (OPD) for four samples

with Tc = 1.65K, 2.9K and 3.5K and 6.4K. We observe that for the sample with Tc =

6.4K OPD peaks around S = 0.4. With increasing disorder this weight gradually shifts

towards zero and also the OPD gets widen. This is the indication of gradual formation

of regions where the superconducting OP is suppressed. We introduce the new scaling

variable,

(8)

where = exp (ln ) and 2 = ln2 S − ln 2. When plotted the probability

distribution for rescaled OP ( Fig. 10(b) ) we see that rescaled OPD for all the samples

Synopsis 35

universality of the OPD The OPD is

also in good agreement with Tracy-

Widom distribution whose relevance

finite dimensions24,25. We also

OPD within two prototype fermionic

and bosonic models for disordered

superconductors26 showing an

excellent agreement between

the local OP.

NbN

In this section we will focus on temperature evolution of domain structure that

is seen at the lowest temperature as the system is driven across Tc into pseudogap state.

At high temperatures coherence peaks get diffused due to thermal broadening and the

h-maps can no longer be used as a reliable measure of the OP distribution. This problem

is however overcome by tracking the zero bias conductance (ZBC) value in the

tunneling spectra to track temperature evolution of domains based on our observation

of weak anticorrelation between h maps and ZBC maps at lowest temperature.

We investigated the temperature evolution of the domains as a function of

temperature for the sample with Tc ~ 2.9 K. The bulk pseudogap temperature was first

determined for this sample by measuring the tunneling spectra at 64 points along a 200

nm line at ten different temperatures. Fig.11(a) shows the temperature evolution of the

normalized tunneling spectra along with temperature variation of resistance. In

0.0 0.2 0.4 0.6 0.8 0

1

2

3

0.2

0.4

0.6

6.4K

3.5K

2.9K

1.65K

TW

distribution for the four samples (b) The

same data as in panel (a) plotted in terms of

the rescaled variable RS. The solid line

corresponds to the Tracy-Widom

36 Synopsis

principle, at the T*, GN(V = 0) GN(V>>/e). Since this cross-over point is difficult to

uniquely determine within the noise levels of our measurements, we use GN(V = 0)/GN

(V = 3.5 mV) ~ 0.95 as a working definition for the T*. Using this definition we obtain

T* ~ 7.2 K for this sample.

Spectroscopic maps were subsequently obtained at 6 different temperatures

over the same area as the one in Fig. 9(e). Before acquiring the spectroscopic map we

0 50 100 150 200

0.3

0.4

0.5

0.6

0.3

0.4

0.5

0.6

0.7

0.3

0.4

0.5

0.6

0.7

0.4

0.6

0.8

0.6

0.8

1.0

0.6

0.8

1.0

Figure 11 Temperature evolution of the inhomogeneous superconducting state

for the sample with Tc = 2.9K. (a) Temperature evolution of spatially averaged

normalized tunneling spectra plotted in the form of intensity plot of GN(V) as a

function of bias voltage and temperature. Resistance vs temperature (R-T) for the same

sample is shown in white curve on the same plot. Pseudogap temperature T* ~ 7.2 K is

marked with the dotted black line on top of the plot. (b)-(g) Spatial variation of ZBC

(GN(V=0)) plotted in the form of intensity plot over the same area for six different

temperatures.

Synopsis 37

corrected for the small drift using the topographic image, such that the maps were taken

over the same area at every temperature. Fig. 11(b)-(g) show the ZBC maps as a

function of temperature. Below Tc, the domain pattern does not show a significant

change and for all points ( = 0) ( = 3.5)⁄ < 1 showing that a soft gap is

present everywhere. As the sample is heated across Tc Most of these domains continue

to survive at 3.6K across the superconducting transition. Barring few isolated points (

< 5% ) the soft gap in the spectrum persist even at this temperature. At 6.9K, which is

very close to T*, most of the domains have merged in the noise background, but the

remnant of few domains, originally associated with a region with high OP is still

visible. Thus the inhomogeneous superconducting state observed at low temperature

disappears at T*.

These observations provides a real space perspective on the formation of the

pseudogap state through phase disordering. Below Tc the coherent superconducting

domains get Josephson coupled giving rise to the global zero resistance state. With

increase in temperature thermal fluctuations cause this coupling to get weaker. At Tc

the weakest coupling is broken and the phase coherence between domains with finite

superconducting OP get lost. However, superconducting correlations within domains

continue to persist up to much higher temperature T* giving rise to the pseudogap state

in tunnelling measurement.

Chapter 5. Summary

In this chapter we discuss the implication of our results on the nature of the

superconducting transition. In a clean conventional superconductor the

superconducting transition, well described through BCS theory, is governed by a single

energy scale, which represent the pairing energy of the Cooper pairs. Consequently,

Tc is given by the temperature where This is indeed the case for NbN thin films

in the clean limit. On the other hand in the strong disorder limit, the persistence of the

gap in the single particle energy spectrum in the pseudogap state and the insensitivity

of on Tc conclusively establishes that is no longer the energy scale driving the

superconducting transition. Indeed, the formation of an inhomogeneous

superconducting state supports the notion that the superconducting state should be

visualized as a disordered network of superconducting islands where global phase

38 Synopsis

superconducting islands. Consequently at Tc, the phase coherence would get destroyed

through thermal phase fluctuations between the superconducting domains, while

coherent and incoherent Cooper pairs would continue to survive as evidenced from the

persistence of the domain structure and the soft gap in the tunneling spectrum at

temperatures above Tc. Finally, at T* we reach the energy scale set by the pairing energy

where the domain structure and the soft gap disappears.

These measurements connect naturally to direct measurements of the superfluid

phase stiffness (J) performed through low frequency penetration depth and high

frequency complex conductivity ( 'i” ) measurements on similar NbN

samples. Low frequency measurements8 reveal that in the same range of disorder where

the pseudogap appears ( Tc ≤ 6K), J(T 0) becomes a lower energy scale compared to

High frequency microwave measurements27 reveal that in the pseudogap regime

the superfluid stiffness becomes strongly frequency dependent. While at low

frequencies J ( ”) becomes zero close to Tc showing that the global phase

coherent state is destroyed, at higher frequencies J continues to remain finite up to a

higher temperature, which coincides with T* in the limit of very high frequencies. Since

at the probing length scale set by the electron diffusion length at microwave

frequencies27 is of the same order as the size of the domains observed in STS, finite J

at these frequencies implies that the phase stiffness continues to remains finite within

the individual phase coherent domains. Similar results were also obtained from the

microwave complex conductivity of strongly disordered InOx thin films28.

In summary, we have demonstrated the emergence of an inhomogeneous

superconducting state, consisting of domains made of phase coherent and incoherent

Cooper pairs in homogeneously disordered NbN thin films. The domains are observed

both in the local variation of coherence peak heights as well as in the ZBC which show

a weak inverse correlation with respect to each other. The origin of a finite ZBC at low

temperatures as well as this inverse correlation is not understood at present and should

form the basis for future theoretical investigations close to the SIT. However, the

persistence of these domains above Tc and subsequent disappearance only close to T*

provide a real space perspective on the nature of the superconducting transition, which

is expected to happen through thermal phase fluctuations between the phase coherent

Synopsis 39

domains, even when the pairing interaction remains finite. However, an understanding

of the explicit connection between this inhomogeneous state and percolative transport

for the temperature above and below Tc is currently incomplete29,30,31 and its

formulation would further enrich our understanding of the superconducting transition

in strongly disordered superconductors.

We finally summarize the evolution of various energy scales as a

function of disorder for NbN. Superfluid stiffness J was measured using two coil

mutual inductance technique and converted to temperature scale using J/kB. is

obtained using the BCS relation,

=

1.76 (9)

where Δ(0) is ground state superconducting energy gap obtained by fitting

tunneling spectra using DOS given by equation (4). It is instructive to note that in the

range of disorder

1

10

100

Figure 12 Phase diagram of for strongly disordered NbN

showing various temperature scales as a function of kFl. Tc is

obtained transport measurement. T* is pseudogap temperature,

J/kB is the superfluid stiffness converted into temperature scale.

is obtained from BCS relation for superconducting

transition temperature and ground state energy gap Δ(0).

40 Synopsis

Phys. Today 51 39 (1998)

3 Sambandamurthy G et al, Phys. Rev. Lett. 94 017003 (2005); Baturina T I et

al, Phys. Rev. Lett, 98 127003 (2007); Nguyen H Q et al, Phys. Rev. Lett.

103 157001 (2009)

4 M. D. Stewart Jr., A. Yin, J. M. Xu, and J. M. Valles Jr.

Science 318 1273 (2007)

5 R. Crane, N. P. Armitage, A. Johansson, G. Sambandamurthy, D. Shahar, and

G. Grüner

Phys. Rev. B 75 184530 (2007)

6 B. Sacépé, C. Chapelier, T. I. Baturina, V. M. Vinokur, M. R. Baklanov, and

M. Sanquer

Nat. Comm. 1 140 (2010)

7 B. Sacépé, T. Dubouchet, C. Chapelier, M. Sanquer, M. Ovadia, D. Shahar,

M. Feigel'man, and L. Ioffe

Nat. Phys. 7 239 (2011)

8 M. Mondal, A. Kamlapure, M. Chand, G. Saraswat, S. Kumar, J. Jesudasan,

L. Benfatto, V. Tripathi, and P. Raychaudhuri

Phys. Rev. Lett. 106 047001 (2011)

9 P. W. Anderson et al, Phys. Rev. B 28 117 (1983); A. M. Finkelstein, Phys. B

197 636 (1994)

11 A. Ghosal, M. Randeria, and N. Trivedi

Phys. Rev. Lett. 81 3940 (1998)

12 Y. Dubi, Y. Meir and Y. Avishai

Nature, 449 876 (2007)

13 K. Bouadim, Y. L. Loh, M. Randeria, and N. Trivedi

Synopsis 41

Nat. Phys. 7 884 (2011)

14 M. Mondal, M. Chand, A. Kamlapure, J. Jesudasan, V. C. Bagwe, S. Kumar,

G. Saraswat, V. Tripathi and P. Raychaudhuri, J. Supercond. Nov. Magn. 24

341 (2011)

15 S. P. Chockalingam, Madhavi Chand, John Jesudasan, Vikram Tripathi and

Pratap Raychaudhuri

Phys. Rev. B 77, 214503 (2008)

16 M. Chand, A. Mishra, Y. M. Xiong, A. Kamlapure, S. P. Chockalingam, J.

Jesudasan, V. Bagwe, M. Mondal, P. W. Adams, V. Tripathi, and P.

Raychaudhuri

Phys. Rev. B 80, 134514 (2009)

17 A. Kamlapure, T. Das, S. C. Ganguli, J. B Parmar, S. Bhattacharyya, P.

Raychaudhuri

arxiv.org/abs/1308.2880 (2013)

18 A. Kamlapure, G. Saraswat, S.C. Ganguli, V. Bagwe, P. Raychaudhuri, S. P

Pai

Mineola, New York, 2004).

Phys. Rev. Lett. 44 1288 (1980).

21 V. J. Emery and S. A. Kivelson,

Phys. Rev. Lett. 74 3253 (1995).

22 M. Chand, G. Saraswat, A. Kamlapure, M. Mondal, S. Kumar, J. Jesudasan,

V. Bagwe, L. Benfatto, V. Tripathi, and P. Raychaudhuri

Phys. Rev. B 85, 014508 (2012)

23 Dynes, R. C., Narayanamurti, V., and Garno, J. P. Direct Measurement of

Quasiparticle-Lifetime Broadening in a Strong-Coupled Superconductor. Phys.

Rev. Lett. 41, 1509 (1978).

24 C. Monthus and T. Garel, J. Stat. Mech.: Theory Exp. P01008 (2012)

25 C. Monthus and T. Garel, J. Phys. A: Math. Theor. 45, 095002 (2012).

26 G. Lemarié, A. Kamlapure, D. Bucheli, L. Benfatto, J. Lorenzana, G. Seibold,

S. C. Ganguli, P. Raychaudhuri and C. Castellani

42 Synopsis

Phys. Rev. B 85 184509 (2013)

27 M. Mondal, A. Kamlapure, S. C. Ganguli, J. Jesudasan, V. Bagwe, L.

Benfatto and P. Raychaudhuri.

Scientific Reports 3, 1357 (2013).

28 Liu, W., Kim, M., Sambandamurthy, G. and Armitage, N. P.

Phys. Rev. B 84, 024511(2011).

29 Bucheli, D., Caprara, S., Castellani, C. and Grilli, M.

New Journal of Physics 15, 023014 (2013).

30 Li, Y., Vicente, C. L. and Yoon, J.

Phys. Rev. B 81, 020505(R) (2010).

31 Seibold, G., Benfatto, L., Castellani, C. & Lorenzana, J.

Phys. Rev. Lett. 108, 207004 (2012).

Chapter 1

The phenomenon of superconductivity was discovered by Heike Kamerlingh

Onnes in 1911 where he observed a sudden drop to zero in the resistivity of Mercury,

to an experimental error, at 4.2K. Soon after, many more materials such as aluminium,

lead, tin etc. showed the superconductivity on cooling. The temperature below which

material turns superconducting is called as critical temperature (Tc). In 1933 it was

found by Walter Meissner and Robert Ochsenfeld that superconductor expels the weak

external applied magnetic field from entering into the bulk. The expulsion of magnetic

field would not take place in perfect conductor of free electrons, showing that the

superconductor is more than just perfect conductor.

Since the discovery of superconductivity, theorists struggled for several

decades to understand the origin of superconductivity although major advances made

through phenomenological theories mainly by London in 1935 and Ginzburg-Landau

Figure 1-1 Basic requirements of superconductivity: (a) Zero resistance state

below 4.2K as discovered by Kamerlingh Onnes in 1911, (b) Meissner- Ochsenfeld effect

showing expulsion of magnetic field below critical temperature

44 Chapter 1. Introduction

in 1950. It is John Bardeen, Leon Neil Cooper, and John Robert Schrieffer (BCS) who

first gave the microscopic theory of superconductivity in 1957. The basic idea in the

BCS theory is that in the superconducting state electrons pair though phonon coupling

and these pairs, called as Cooper pairs, condense into a single phase coherent ground

state which allows the electrons to move without scattering.

For the obvious technological reasons search for the new materials which could

superconduct at higher temperatures continued and in 1986 Alex Müller and Karl

Bednorz discovered a new class of superconductor known as the doped rare earth

cuprates. These materials become superconducting above 30K. In following years a

host of new material were found which superconduct at temperatures much higher than

the boiling point of liquid N2. These new class of materials are called as high

temperature superconductors (HTSC). Not much progress is made in understanding the

origin of HTSC although there are theories which qualitatively explain the possible

mechanism of pairing and symmetry of the gap.

While the quest for new materials continued, there have been also the

investigations by some researchers on the effect of disorder on superconducting

properties of the material. The problem gives a unique opportunity to study the

competition between superconductivity which results from pairing and the pair

breaking effects of electron localization and disorder induced Coulomb repulsion. The

interest in the field was further increased by the possibility that the disorder driven or

magnetic field driven suppression of superconductivity in the limit of zero temperature

might be a quantum phase transition.

In this thesis we study the effect of disorder on superconducting properties of

s-wave superconductor, NbN, close to metal insulator transition. The study was mainly

carried out using home built low temperature Scanning Tunneling Microscopes (STM).

The plan of the introduction chapter is as follows. In the first section I will describe the

basics of superconductivity and essential concept required to make platform for our

study. I will then review the experimental and theoretical advances in the field of

disorder/ magnetic field driven superconductor insulator transition (SIT). I will finally

introduce to our model system NbN and its characterization through transport

measurements and transmission electron microscopy (TEM).

Chapter 1. Introduction 45

1.1 Basics of Superconductivity

1.1.A The Meissner-Ochsenfeld effect

When a superconductor is cooled below its Tc and kept in a weak external

magnetic field then it expels the magnetic flux lines from entering into the bulk so that

the field inside a superconductor is zero (B = 0). This phenomenon is called as

Meissner-Ochsenfeld effect. Although superconductors show the perfect diamagnetism

at low fields, strong magnetic fields destroy the superconductivity. The field at which

superconductivity breaks down is called as the critical field (Bc)

1.1.B The London equations

The phenomenological theory developed by London brothers1 in 1935 explains

the perfect conductivity as well as the Meissner effect where they showed that the

superconductor produces screening current at the surface which shields the external

magnetic field from entering into the bulk. The two equation governing electromagnetic

fields inside a superconductor are,

= 2

The first equation essentially explains the perfect conductivity through the free

acceleration of charge. Using the identities in vector calculus and Amperes law one can

deduce the second equation to,

∇2 = 1

2 (1.3)

Where is called as London penetration depth and is defined as,

= √ 2

42 (1.4)

One can immediately see that on application of magnetic field = to

semi-infinite superconductor (Figure 1-2), the magnetic field inside the superconductor

is given by

46 Chapter 1. Introduction

Figure 1-2 The boundary between superconductor and magnetic field. Blue curve

inside the superconductor shows exponential fall characterized by London penetration

depth λL. Orange curve show the dependence of the current density with distance inside

the superconductor.

() = − ⁄ for x ≥ 0 (1.5)

i.e. the magnetic field inside the superconductor decreases exponentially and in

the bulk we find B → 0, hence the Meissner effect. Also from the second London

equation (Equ. 1.2) along with equation of continuity (∇ = 0) it follows that,

() = −

− ⁄ for x ≥ 0 (1.6)

Thus the supercurrents flow in the direction parallel to the surface and

perpendicular to B and decrease into the bulk over the same scale .

1.1.C Nonlocal Response: Pippard Coherence length ( ξ0 )

The nonlocal generalization of the London equations was proposed by Pippard2.

He argued that the superconducting wavefunction has a characteristic dimension ξ.

Superconducting properties such as superfluid density changes over the length scale of

ξ which can be estimated using uncertainty principle and is given by,

Chapter 1. Introduction 47

ξ =

(1.7)

Where α is a numeric constant of the order of unity. BCS theory predicts that

the value of α ≈ 0.18. It also has a physical significance in BCS theory that it represents

the size of the Cooper pairs.

1.1.D Ginzburg Landau (G-L) model of superconductivity

The phenomenological theory of superconductivity was introduced by

Ginzburg and Landau3 in 1950 which describes superconducting phase transition

within Landau’s general theory of second order phase transition. They introduced a

complex pseudo-wave function = || as an order parameter to describe

superconducting electrons.

G-L equation can be obtained using the variational principle to minimize the

free energy and it has the form analogous to Schrodinger’s equation,

1

= ∗

∗2

∗ ||2 (1.9)

With = || and using equ. 1.8 we can get the equation for supercurrent

velocity as,

=

2 (∇ −

) (1.10)

It can be shown that G-L order parameter can be related to local density of

superelectrons as,

Phase stiffness

Bulk superconducting ground state is described by a constant order parameter,

, where the phase of the order parameter, , has a constant value everywhere. There

is an energy cost associated with changing from one part of the superconductor to

another. This energy cost is called as phase stiffness or superfluid stiffness and denoted

as J. From equ. 1.10, the velocity of the superfluid is given by,

=

2 (∇φ) (1.12)

Now the increase in kinetic energy by phase twist is given by

∫ 3 (

4 ∫3(∇)2. In analogy with XY model4,5 in statistical

physics we define J over the cut-off distance as6,7,

= 2

4 (1.13)

For all our analysis we take the minimum cut-off distance a equal to coherence

length ξ as it is a characteristic length scale over which the superconducting parameters

changes. It is important to note that ∝ which is related to λL (equ. 1.4) which is

experimentally measureable quantity.

Solving G-L equation at the interface of superconductor introduces a

characteristic length called as G-L coherence length given by = ( 2

2∗|()| ) 1 2⁄

and it

is the measure of the distance over which order parameter respond to a perturbation.

To the first order approximation in α, it can be written as, () = (0)||−1 2⁄ , where

= −

= √ 2

82 (− ) (1.14)

Chapter 1. Introduction 49

The ratio =

is called as G-L parameter is an important parameter and is

independent of temperature within G-L theory.

Type I and Type II superconductors

The superconductors with G-L parameter < 1

√2 are called as Type-I

superconductors. These materials show a perfect diamagnetism at all fields below a

critical field Hc where the superconductivity is completely destroyed. Most elemental

superconductors are Type-I superconductors. In 1957 Abrikosov8 showed that for

superconductors with > 1

√2 , there exist an equilibrium state in presence of magnetic

field where the field lines penetrate the superconductors to form vortices. These

materials are called as Type-II superconductors. Vortices in Type-II superconductors

are formed above the lower critical field Hc1 and there is continuous increase in the flux

penetration till the upper critical field Hc2 where the superconductivity is completely

destroyed.

These vortices in Type-II superconductors form a triangular lattice9 and each

vortex contains exactly one quantum of flux, Φ0 = 2⁄ = 2.07 × 10−15 Wb. The

nearest neighbour distance for the vortex lattice is given by,

= 1.075 ( Φ0 ) 1 2⁄

(1.15)

Figure 1-3(a) shows the contour diagram for ||2in presence of magnetic field for

Figure 1-3 Abrikosov Flux lattice: (a) theoretically calculated contour diagram of

|| just below the upper critical field (b) triangular lattice of flux lines on the surface of

Pb. The black dots are cobalt particles.

50 Chapter 1. Introduction

type-II superconductor. Figure 1-3(b) shows the results of first experiment to visualize

the vortex lattice10.

Microscopic theory of superconductivity given by Bardeen, Cooper and

Schrieffer11 (BCS) in 1957 explains the superconductivity in many metals and predicts

many properties. The idea behind the theory is that ground state of free electrons is

unstable against the small attractive interaction between electrons12, no matter how

small is the interaction and the electrons pair to form bound state. The attractive

interaction between the electrons is provided by electron phonon exchange which can

be understood as follows: an electron with negative charge –e attracts the positively

charged ions as it moves in the crystal and the lattice distortion locally induces

excessive positive charge. This positive charge is in turn attracts another electron

forming a bound state with the first one. The cartoon picture showing the phonon

mediated attraction is as shown in Figure 1-4.

Figure 1-4. Cartoon picture of Cooper pair, pair of electrons with equal and

opposite momenta.

Cooper showed in that the bound state energy of the electron pair with equal

and opposite momenta and spin is given by,

ε = −2ω −(2 (0)⁄ ) (1.16)

Chapter 1. Introduction 51

where is the cut-off frequency corresponding to the Debye temperature. Next

we will briefly review the BCS theory11.

BCS took the form for the ground state as,

| = ∏ ( + ↑ + −↓

+ )|0

Where || 2 + ||

2 = 1 and |0 is the vacuum state. Coefficients and

are chosen so as to minimize the expectation value of the energy using the so called

reduced Hamiltonian,

−↓ + −↓↑ (1.17)

BCS assumed the simple form for the attractive interaction as,

= { −, |ξ|and |ξ| ≤ ω 0, Otherwise

(1.18)

Where ξ is the single particle energy of the electrons with respect to Fermi

energy. Following are the important key results of BCS theory,

The gap function

Δ(0) = 2ω −1 (0)⁄ (1.19)

Where Δ is the superconducting energy gap formed at the Fermi level and (0)

is Fermi level density of states.

Temperature dependence of the gap and Tc

Temperature dependence of the gap can be numerically calculated using,

1

(0) = ∫

(2 + Δ2)1 2⁄

ω

0

(1.20)

where = () −1. Figure 1-5 shows the temperature dependence of which

holds in good approximation for most of the conventional superconductors.

52 Chapter 1. Introduction

The critical temperature is the temperature at which Δ() → 0. Thus the integral

1.16 can be evaluated by substituting Δ = 0 and it yields,

= 1.13ω −1 (0)⁄ (1.21)

Comparing with Equ. 1.15 we get,

Δ(0) = 1.764 (1.22)

Figure 1-5. Temperature dependence of energy gap within BCS theory.

BCS density of states

The quasiparticles excitation energy within BCS theory is given by 2 =

2 + 2 which shows the minimum excitation to be i.e. there is a gap in the energy

spectrum. The single particle density of states (DOS) is given by,

()

Chapter 1. Introduction 53

Figure 1-6. Density of states in superconducting state compared to the normal

state.

1.1.F Electron tunneling and measurement of

In 1960 Giaever13 introduced a method to measure the for the superconductor

based on the principle of quantum mechanical tunneling. The measurements involves

tunnel junction which consists of a normal metal and a superconductor separated by

very thin insulating layer. The tunneling current between normal metal and a

superconductor is given by,

∞

−∞

(1.24)

Where 2() is the BCS density of states and f is the Fermi function. More

direct comparison between theory and experiments can be made through the tunneling

differential conductance,

(1.25)

It can be seen that as → 0 the tunneling conductance mimics the density

of states for the superconductors,

54 Chapter 1. Introduction

2(0) (1.26)

Figure 1-7(a) shows the tunneling differential conductance spectra plotted as a

function of V for the NbN-oxide-Ag tunnel junction at various temperatures14. Solid

lines shows the fits using BCS density of states (Equ. 1.18) with additional broadening

parameter Γ which takes into account the additional broadening due to finite lifetime

of the superconducting quasiparticles15.

() = ( || + Γ

√(|| + Γ)2 − Δ2 ) (1.27)

Figure 1-7(b) shows the temperature evolution of and Γ plotted along with

resistivity Vs temperature curve.

0.5

1.0

1.5

2.0

2.5

0.0

0.4

0.8

1.2

1.6

0.2

0.4

0.6

0.8

1.0

m

Figure 1-7. Tunneling measurements on NbN/oxide/Ag planar tunnel junction with Tc =

14.9K. (a) G(V)-V spectra at different temperatures along with the BCS-Γ fits, (b)

Temperature dependence of , Γ and ρ.

1.2 Disordered Superconductors

The interplay of superconductivity and disorder is one of the most intriguing

problems of quantum many body physics. Superconducting pairing interactions in a

normal metal drives the systems into a phase coherent state with zero electrical

resistance. In contrast, in a normal metal increasing disorder progressively increases

the resistance through disorder scattering eventually giving rise to an insulator at high

disorder where all electronic states are localized. Quite early on, it was argued by

Anderson16 that since BCS superconductors respect time reversal symmetry,

Chapter 1. Introduction 55

superconductivity is robust against nonmagnetic impurities and the critical temperature

Tc is not affected by such disorder. Anderson’s idea however applies only to weakly

disordered systems, with their extended electronic states. In presence of strong disorder

experiments showed that it reduces Tc and ultimately drives the system into an

insulator17,18,19,20. This suppression of superconductivity could be thickness

driven21,22,23, magnetic field driven24 or disorder driven25,26. Various other novel

phenomena are observed in the vicinity of superconductor insulator transition (SIT).

The two key observations are (i) persistence of finite superconducting correlations

above Tc through measurements of finite high J stiffness above Tc in amorphous InOx

films27,28, finite spectral gap at zero bias in the conductance spectra much above Tc in

scanning tunneling microscope (STM) experiments29,30,31 etc., and (ii) presence of

superconducting correlations/ Cooper pairing through the measurements of activated

temperature dependence of resistance on the insulating side32, the giant peak in the

magnetoresistance in thin films33,34,35, magnetic flux quantization in nano-honeycomb

patterned insulating thin films of Bi36, a more recent transport37,38 and tunneling

experiments39.

Although the complete theoretical understanding of the nature of SIT is lacking,

in recent times numerous theoretical and numerical advances have been made. It is

shown that in the intermediate disorder limit the effect of disorder is to decrease the

pairing amplitude40,41 through an increase in the electron-electron (e-e) Coulomb

repulsion which results in decrease in Tc. In presence of strong disorder experimental

observations are understood qualitatively through number of prototype models of

disordered superconductors which are based on either fermionic42,43,44,45,46 or

bosonic47,48,49 description. The fermionic models demonstrated the survival spectral

gap across SIT and the transition is driven by phase fluctuation between

superconducting islands. Bosonic models indicated that the SIT is driven by quantum

phase fluctuations between localized Cooper pairs.

In particular here I would like to highlight on the recent numerical simulations

which have direct relevance to the work presented in this thesis. These simulations

involve solving Attractive (negative-U) Hubbard model with random on-site

energy43,50,45. While these studies ignore Coulomb interactions and are done on

relatively small systems compared to real superconductors, they nevertheless support

56 Chapter 1. Introduction

key aspects of the basic scenario of the disordered superconductors namely (i) Single

particle spectral gap in the DOS at lowest temperature survives through SIT and is finite

everywhere though it is highly inhomogeneous. However J, decreases rapidly with

increasing disorder making the system more susceptible to phase fluctuations. (ii)

Coherence peak heights at the gap edge are directly correlated to the local

superconducting order and vanish with increasing temperature and disorder. (iii) Near

SIT, pseudogap appears in the DOS at low energies above Tc and also on the insulating

side. These results are indeed in good agreement with our results on disordered NbN

presented in this thesis.

In spite of the fact that the field of disordered superconductors has produced

variety of novel phenomena and interesting theoretical results which has enriched our

understanding of SIT to a great extent, more experimental works are needed for

complete understanding and resolving the open questions in the field. More

specifically, in regard of theoretical propositions, suggesting the emergence novel

phenomena beyond the ambit of BCS theory, there is very little direct experimental

evidence confirming the predictions made. In this thesis we address most of the

experimental remedies through our investigation on NbN which can be grown with

larger atomic defects by tweaking growth parameters.

1.3 Our model system: NbN

For our investigation we use NbN as a model system to study the effect of

disorder. NbN is a conventional s-wave superconductor with optimum Tc ~ 17K. Bulk

NbN has the λ of ~ 250 nm, electronic mean free of l ~ 4nm and the ξ ~ 5nm. It has

face centred cubic structure similar to NaCl. Band structure calculations show that

Fermi level lies within the 4d band and these electrons contribute to the conduction.

1.3.A Sample growth and introducing disorder

Epitaxial thin films of NbN are grown using reactive DC magnetron sputtering

in Ar+N2 gas mixture on (100) oriented single crystalline MgO substrate which is

heated to 600°C. The optimum conditions to get the highest Tc of 17K are sputtering

power =200W, Ar:N2 ratio = 84:16. The disorder in the system is tuned by varying

deposition conditions: either by decreasing the sputtering power keeping the partial gas

pressures constant or by increasing the N2 partial pressure51,52. In both these cases Nb

Chapter 1. Introduction 57

flux relative to N2 in the plasma is reduced which results in the Nb vacancies in the

crystal hence the disorder. For our study all the films are deposited with thickness ≥

50nm which is much larger than the dirty limit coherence length ~5-8 nm53 and can

be considered to be 3D as far as superconducting correlations are concerned.

1.3.B Structural characterization of NbN films

X-ray diffraction (XRD) study on films grown using above method show the

formation of crystalline NbN on MgO substrates54. All our films show high degree of

epitaxy as seen from the -scans using a four circle goniometer. This is further

confirmed directly through the high resolution transmission electron microscope

(HRTEM). Figure 1-8(a) and (b) show HRTEM images probed at the interface of

MgO

1 nm

Figure 1-8 TEM images (a), (b) High resolution TEM images for two samples

with Tc ~ 16K and 2.5K at the interface of NbN-MgO. (c), (d) corresponding high

resolution scanning TEM images.

substrate and NbN film along <110> direction for the two samples with Tc ~ 16K and

2.5K respectively. The difference between two samples at the atomic scale is revealed

58 Chapter 1. Introduction

in Figure 1-8(c) and (d) which shows the high resolution scanning transmission

(HRSTEM) images for same samples respectively. Intensity in the HRSTEM image is

primarily contributed by Nb and is proportional to the number of Nb atoms in the

probing column. Smooth intensity variation in clean sample (Tc ~ 16K) shows the

overall thickness variation produced during ion beam milling while the disordered

sample (Tc ~ 2.5K) shows random distribution of intensity in the columns showing

random number of Nb atoms in the adjacent columns. This clearly shows that for the

disordered films, the lattice contains Nb vacancies but when probed at the large scale

it is homogeneous. Thus we have an ideal system in which disorder is present at the

atomic length scale and the disorder is homogeneous over entire film.

1.3.C Quantification of disorder

To quantify disorder we use the Ioffe Regel parameter which is the measure

of mean free path in units of de-Broglie wavelength (). In clean system and

therefore has a large value. With increasing disorder decreases steadily due to

disorder scattering and therefore the quantity also decreases. At ≤ 1 all the

bloch states are completely localized which corresponds to Anderson metal insulator

transition (MIT). values are extracted from resistivity and Hall measurements and

calculated using free electron formula,

= (32)2 3⁄ [(285)]

1 3⁄

(285)5 3⁄ (1.28)

Here = − 1

assumes absence of e-e interaction which is not the case for

our disordered samples. Therefore we calculate at highest temperature of our

measurements (i.e. at 285K) where the effects of interaction is believed to be smaller55.

in our samples ranges from 10 (Tc = 16K) to all the way down to 0.42 (Tc < 300mK)

and we observe that ~ 1 is the critical disorder where superconductivity is

completely destroyed.

1.4 Effects of disorder

In this section we will review our recent work on disordered NbN through the

transport and λ measurements.

Chapter 1. Introduction 59

1.4.A Resistivity and measurement of Tc

Figure 1-9(a) shows resistivity Vs temperature curves ( − ) for full range of

disorder. The inset of Figure 1-9(a) shows the expanded view of − in the transition

region. Figure 1-9(b) shows the plot of Tc values with increasing disorder, Tc being the

temperature at which resistivity becomes 1% of its normal state value. Here we see that

→ 0 as → 0. Most disordered samples with < 1 do not show

superconducting downturn all the way down to 300mK. For these samples Tc is taken

as 300mK. From − curves we observe that except the least disordered sample with

= 10.12, all the samples show negative temperature coefficient which gets more

and more pronounced with increasing disorder.

50 100 150 200 250 300 10

-1

4

8

12

16

200

400

600

800

1000

0 2 4 6 8 10 12 14 16 18 20 10

-1

T (K)

Figure 1-9. (a) ρ – T for NbN films with different kFl, the inset shows the

expanded view in the transition region. (b) Variation of Tc with kFl, (c) Conductivity σ –

T at low temperature for the three samples with kFl = 0.82, 0.49 and 0.42. Extrapolations

to σ as → are shown with lines of different colour.

60 Chapter 1. Introduction

Figure1- 9(c) shows the conductivity Vs temperature − curves for three

most disordered samples with < 1. When extrapolated as → 0 the has finite

value which implies that our most disordered samples are not insulators but are bad

metals. Conventionally = 1 is associated with Anderson metal insulator transition.

The inconsistency between values and the observed metallic behaviour shows that

in presence of strong e-e interaction free electronic theory cannot be applied to measure

accurately values.

1.4.B Hall carrier density measurement

Carrier density (n) for the samples with various disorder is obtained by Hall

resistance measurement. Figure 1-10(a) shows plotted as a function of applied

magnetic field. Carrier density n is given by = −1 ⁄ where , the Hall

coefficient is extracted from the slope of − curves. Above relation for n is valid

only in the absence of e-e interactions therefore n is determined at 285K following

argument from section x. The measured carrier density for the stoichiometric NbN with

Tc ~ 16K is in good agreement with the band structure calculations56. Figure 1-10(b)

shows the n(285K) for films with increasing disorder.

0 4 8 12 -2.0

-1.5

-1.0

-0.5

0.0

5

10

15

20

25

0.49

0.82

1.68

3.27

5.5

k F l

Figure 1-10. Hall measurements, (a) ρxy – H measured at 285K for samples with

different kFl. (b) carrier density n extracted from ρxy and plotted as function of kFl.

Chapter 1. Introduction 61

1.4.C Upper critical field (Hc2) and coherence length (ξGL)

Figure 1-11 shows experimentally measured Hc2 and ξ for samples with varying

levels of disorder. We observe the non-monotonic behaviour in these quantities with

increasing disorder which can be

Recommended